USE OF FINITE ELEMENT METHOD TO EVALUATE THE STRENGTH RESPONSE OF NOTCHED COMPOSITE LAMINATES UNDER TENSION ARJUN KOTHIDAR


 Clemence Porter
 1 years ago
 Views:
Transcription
1 USE OF FINITE ELEMENT METHOD TO EVALUATE THE STRENGTH RESPONSE OF NOTCHED COMPOSITE LAMINATES UNDER TENSION By ARJUN KOTHIDAR A thesis submitted in partial fulfillment of the requirements for the degree of MASTER OF SCIENCE IN MECHANICAL ENGINEERING WASHINGTON STATE UNIVERSITY Department of Mechanical and Materials Engineering December 008
2 To the Faculty of Washington State University: The members of the Committee appointed to examine the thesis of ARJUN KOTHIDAR find it satisfactory and recommend that it be accepted. Chair ii
3 ACKNOWLEDGEMENT I would like to thank my advisor, Dr. Lloyd V. Smith, for providing me the opportunity to work on this project. He has provided the resources, encouragement and freedom to explore, and his expertise and counsel are greatly appreciated. In addition, thanks are due to my thesis committee, Dr. JowLian Ding and Dr. Vikram Yadama who have been very patient and supportive throughout my work. I would like to thank Daniel P. Stone, my project partner for this project for all his work and discussions. Thanks to Miles Peppers and Henry Ruff for their assistance in the area of composite fabrication. Thank you to the MME staff, including Mary Simonsen, Bob Ames, Gayle Landeen and Robert Lentz whose helpful nature made life really easy during the course of my study. I d like to thank Giac Pham and Micheal Shook for their help and competence with technical issues. Thank you to all the undergraduate students of ETRL 1 LAB who have helped me throughout this project, including Brian Seater, Tyler Start, Matthew Jorgensen and Alex Butterfield. Lastly, and most importantly I would like to thank my family who have been very encouraging throughout my years of learning. iii
4 USE OF FINITE ELEMENT METHOD TO EVALUATE THE STRENGTH RESPONSE OF NOTCHED COMPOSITE LAMINATES UNDER TENSION Abstract by Arjun Kothidar, M.S. Washington State University December 008 Chair: Lloyd V. Smith Mechanical attachments can reduce the strength of composites substantially. The following considers the sensitivity of openhole tension (OHT) test coupons to the laminate fiber orientation. Fiber orientation affects the stress distribution around the hole which can lead to improved laminate strength. The effect of the hole on the OHT strength was described numerically by using a 3D Finite Element (FE) model. The linear elastic model was used to predict the first ply failure (FPF). Maximum Stress and Maximum Strain failure criteria were found to correlate well with the measured FPF strength and location as verified by SEM. The results of the 3D model were used with Quadratic Delamination Criterion. The procedure was successful in identifying laminates with delamination failure modes as identified through SEM. An FE based Representative Volume Element (RVE) has been used to evaluate the homogenized elastic properties of a graphite/epoxy composite material from its constituent properties. The model agreed well with the experimentally obtained elastic properties of the composite lamina. The FE based RVE model approach was found to be iv
5 an improvement over the existing analytical and semiempirical methods, as a single model could be used to generate all the elastic properties of the composite material. v
6 TABLE OF CONTENTS Page ACKNOWLEDGEMENT...iii ABSTRACT... iv LIST OF TABLES... ix LIST OF FIGURES... x CHAPTER 1 LITERATURE REVIEW Introduction Terminology Effect of fiber orientation on stress concentration Stress Analysis Effect of stacking sequence on the strength Net tension strength Delamination strength Failure Criteria study Modebased Quadratic Failure Theories Applicability of Laminate Failure Theories FEA Study Conclusion D FEA MODEL Introduction... 5 vi
7 . Laminate Geometry Material Properties Model Formulation Model Validation Double Notch Shear Test Results Chapter Summary MANUFACTURING Fabrication SEM Sample Preparation DELAMINATION Introduction Finite Element Comparison Notch Effect Results Quadratic Delamination Criterion Chapter Summary COMPUTATIONAL MICROMECHANICS Introduction Numerical Homogenization RVE Geometry Material Properties Boundary Conditions vii
8 5.6 FE Code Implementation Model Validation Chapter Summary CONCLUSION REFERENCES APPENDIX A1 Recovery shear strain Vs recovery time A Code for linear elastic analysis of 1/8 th notched composite plate A3 Strain Vs X distance A4 Macro to calculate volume averaged stress in ANSYS viii
9 LIST OF TABLES 1..1 Stacking sequence of some of the commonly known laminates [3] Stacking sequence of group 1 and group [18] Material property of T600:1533 carbon/epoxy Material property of Aluminum 7075[43] K t optimized layups FPF strength values for K t optimized laminates using DICM and 3D failure criteria Final set of fabricated laminates along with the method of optimization Mode of first ply failure along with the ply failed Delamination initiation stress along with the interfaces delaminated Elastic properties of constituent fibers and matrix of T600:934 composite Material [34] Elastic properties of T300:934 (graphite/epoxy) composite material by using experimental methods and RVE model for a fiber volume fraction of ix
10 LIST OF FIGURES 1..1 Orthotropic lamina with principal and nonprincipal coordinate system [3] Multidirectional laminate with reference (nonprincipal) coordinate system Effect of fiber orientation on stress concentration in a unidirectional laminate [17] Effect of fiber orientation on stress concentration in a crossply laminate [17] Effect of fiber orientation on stress concentration in angleply laminate [17] Effect of fiber orientation of offaxis plies on stress concentration in [ 0 / ±β / 90] s laminates [17] Comparison of nettension strength between open and filledhole laminates [18] Effect of stacking sequence on the through thickness distribution of interlaminar stress σz near the free edge Isochromatic fringe patterns in photoelastic coating around the hole in boron/epoxy specimens of two different stacking sequences [19] Failure patterns of boron/epoxy tensile panels with holes of two different stacking sequences [19] Geometry of laminated plate along with the model geometry Shear stress Vs Shear strain curve for cyclic loading and unloading of ( ± 45) 3 s laminate Viscoelastically recovered Shear Strain Vs Shear Stress Shear Stress Vs Shear Strain for defining Yield Stress Geometry used for FEA study Individual volumes representing each lamina through the thickness Solid 64 element used for the FE model (a) Preliminary mesh of Baseline laminate with 307 elements (b) Refined mesh of Baseline laminate with 5596 elements x
11 .4.5 Comparison of longitudinal direction (y) strain contours for meshes (a) and (b) of Fig Stress P is acting along y direction Variation of longitudinal direction strain at point A ( ε ya ) with increase in number of elements Variation of longitudinal direction strain at point B ( ε yb ) with increase in number of elements (a) Through thickness mesh with one element per ply (b) Mesh with two elements per ply (a) Longitudinal direction strain contour of Baseline laminate for mesh with one element per ply (b) Longitudinal direction strain contour of Baseline laminate for mesh with elements per ply Longitudinal direction strain ( ε y ) contour of 3D model having Aluminum 7075 properties (a) Through the thickness variation of longitudinal direction strain at location A (ε YA ). (b) Through the thickness variation of longitudinal direction strain at location N (ε YN ) Variation of longitudinal and transverse direction strain of baseline laminate through the thickness Strain concentration factor vs hole diameter to width (d/w) ratio for Aluminum Comparison of longitudinal direction strain distribution between 3D FE model and analytical solution for stress state around the hole for baseline laminate (a) Geometry of double notch coupon (b) FE model geometry of double notch coupon (a) FE mesh of the double notch test specimen (b) Interlaminar shear strain ( ) ε 13 contours of the double notch test specimen Variation of interlaminar shear strain ( ε 13) along the gauge length (L) from A to B Variation of interlaminar normal strain ( ) 3 ε along the gauge length (L) from A to B xi
12 .6.5 Interlaminar and normal stress in unclamped double notch coupon [46] Clamped double notched coupon under compressive load [46] Interlaminar and normal stress in clamped double notch coupon [46] (a) Variation of longitudinal direction strain (ε y ) along X direction using D and 3D FE model for Aluminum properties (b) Variation of longitudinal direction strain (ε y ) along Y direction using D and 3D FE model for Aluminum properties (a) Variation of longitudinal direction strain (ε y ) along X direction using D and 3D FE model for T600:1533 properties. (b) Variation of longitudinal direction strain (ε y ) along Y direction using D and 3D FE model for T600:1533 properties Comparison of strength response of laminates using K t and UTS Load strain curve for uniaxially loaded laminate showing multiple ply failures leading up to ultimate laminate failure[34] Comparison of predicted and measured stressstrain response of [ 0 / ± 45 / 90] s glass/epoxy laminate [34] Set up of the DICM instrument (a) Speckle pattern near the hole of Baseline laminate (b) Longitudinal strain profile of 3D model near the hole of baseline laminate at 70.5 Ksi (90 % UTS) Steps in extraction of strain field in DICM (a) DICM speckle pattern of baseline laminate with circular offset zone (b) Longitudinal strain contour of baseline at 13 Ksi (18% UTS) (c) 3D model mesh of baseline laminate (d) longitudinal strain contour of 3D FE model of baseline at 13 Ksi (18% UTS) (a), (b) Longitudinal strain contour for ( ± 45) 4 at 7.5Ksi (41% UTS) using s DICM & 3D FEA respectively (c), (d) Longitudinal strain contour for A laminate at 9Ksi (13% UTS) using DICM &3D FEA respectively) (a), (b), (c) Comparison of 3D FEA with DICM for longitudinal, transverse and inplane shear strain respectively along X direction of the hole for BL DICM Vs 3D FEA for laminate A Applied stress Vs Longitudinal strain for set of Baseline laminates [46] FE mesh of oneeighth model near the edge of the hole for baseline laminate xii
13 .7.15 Comparison of FPF strength of Kt optimized laminated using DICM and failure theories Comparison of FPF of laminates optimized using MaxStrain theory with DICM Failure Indices (f.i) Vs X distance along the hole at the lamina location where FPF is predicted in transverse mode Failure Indices (f.i) Vs X distance along the hole at the lamina location where FPF is predicted in inplane shear mode Crack in the 90 degree ply of baseline laminate in direction at FPF Crack in the 45 degree ply of H laminate in 1 direction at FPF Trend followed by FPF and UTS of laminates Schematic of fabrication set up [50] Steps in preparing SEM sample for FPF and Delamination study Pipes and Pagano model for analysis of interlaminar stresses in a laminate under uniaxial tension [51] Distribution of stress in free edge region by elasticity method [51] / 45 / 45 / 45 s laminate Geometry and BCs used for FEA of unnotched [ ] 4... Distribution of stresses in the free edge region by FEM for [+45 0 /45 0 /+45 0 /45 0 ] S Predicted variation of interlaminar normal stress field along y [5] Variation of interlaminar normal stress along x for different b/h ratios Interlaminar strain comparison between notched and unnotched coupon Edge of the hole near the point of maximum strain concentration Comparison between FPF, UTS and Delamination initiation stress of different layups Comparison of interlaminar strains between Baseline and G laminate xiii
14 Crack between the 45/90 degree layer in baseline laminate Crack between the 1/90 degree interface in baseline laminate G laminate at ultimate load Laminate A at ultimate load Laminate E at ultimate load Random distribution of fibers in 90 degree lamina in baseline laminate Composite material with a hexagonal array of fibers [58] Geometry of RVE Coordinates of six faces on the RVE block Displacement BC on faces (a 1, x, y) and (a 1, x, y) Displacement BC on faces (z,a, y) and (z, +a, y) Displacement BC on faces (+a 1, x, y) and (a 1, x, y) and faces (z, a, y) and (z, +a, y). Top face showing the shear effect in 1 plane Flow chart for the RVE model Full model of RVE (a) Comparison of longitudinal modulus predicted by rule of mixtures (ROM) model with RVE model (b) Comparison of Poisson s Ratio predicted by rule of mixtures (ROM) with RVE model (a) Comparison of Transverse Modulus predicted by HalpinTsai and TsaiHahn model with the RVE model (b) Comparison of Shear modulus predicted by HalpinTsai and TsaiHahn with the RVE model xiv
15 1. Literature Review 1.1 Introduction An important problem when designing with composites is that of stress concentrations arising near discontinuities. Knowledgee of the magnitude and extent of stress concentrations in these structures is crucial for determining the location of first failure and subsequent damage propagation [1]. This work aims to establish the importance of matrix induced failure in form of the first ply failure in the design of notched laminated composites. 1.. Terminology A lamina or ply is a plane (or curved) layer of unidirectional fibers or woven fabric in a matrix. In the case of unidirectional fibers, it is also referred to as unidirectional lamina (UD). The lamina is an orthotropic material with principal material axes in the direction of fibers (longitudinal), normal to the fibers in the plane of lamina (inplane transverse) and normal to the plane of the lamina. The principal axes are designated as 1, and 3 respectively as shown in Fig Fig Orthotropic lamina with principal and nonprincipal coordinate system [3] Fig.1.. Multidirectional laminate with reference (nonprincipal) coordinate system [3] A laminate is made up of two or more unidirectional laminae or plies stacked together at various orientations as shown in Fig.1... The laminae can be of various thicknesses and consist of 1
16 different materials. Since the orientation of the principal material axes varies from ply to ply, sometimes it is convenient to analyze laminates using a common reference coordinate system (x, y, z). The orientation of a ply is given by the angle between the reference and the major principal material axis measured in a counter clock wise direction on the xy plane as shown in Fig The configuration of the laminate indicating its ply composition is called a layup. The configuration indicating, in addition to the ply composition, the exact location of the various plies is called the stacking sequence. Composite laminates are designated in a manner indicating the number, type, orientation and stacking sequence of plies. Some of the commonly used laminate configurations along with their names are provided in Table 1..1[3]. Table 1..1 Stacking sequence of some of the commonly used laminates [3] Nomenclature Stacking Sequence 0 / 0 / 0 / 0 / 0 / 0 = 0 6 Unidirectional sixply [ ] Cross Ply [ 0 / 90 / 90 / 0] = [ 0 / 90] s Angleply symmetric [ β β β β] = [ ± β] / / / s Angleply asymmetric [ β β β β β β] = [ ± β] [ 0 / β / β / β / β / 0] = [ 0 / ± θ] Multidirectional / / / / / 3 [0 / β / β / 90 / 90 / β / β / 0] = [0 / ± θ / 90] s s In Table 1..1 β is the ply angle that has values between 0 and 90 degrees and s indicates symmetric sequence. The slash mark is used to indicate separate lamina orientations with the subscript indicating the number of laminae of the same orientation. The laminae are specified with the one next to the mold surface written first [4]. The laminates used for this thesis are symmetric and balanced. Symmetric laminates are specified by listing only top half of the laminate and by using the subscript s outside the brackets. A laminate is balanced if it consists of pairs of layers with identical thickness but having + (plus) and (minus) β orientation of their
17 principal material axes with respect to the laminate principal axes. This prevents warpage or unexpected distortions, after the cure cycle is complete and reduces interlaminar stresses. 1.3 Effect of fiber orientation on stress concentration Investigators [513] have used two basic approaches to address the problem of stress concentration around circular cutouts in composite plates. In one approach [15] the problem has been treated analytically by the theory of linear anisotropic elasticity as developed by Lekhnitskii [14]. Based on this approach models have been developed to predict the effect of the notch size on the tensile strength of composites [1517]. In another approach [101], numerical methods such as finite element analysis have been employed. Greszezuk [7] observed that the strength of the composite plates with cutouts is less sensitive to the stress concentration than plates made of isotropic materials. Tan [5] observed that the stress concentration factor in graphite/epoxy angleply laminates could be greater than that of the isotropic case depending on the fiber orientation. Whitworth, H.A. and Mahase, H. [17] investigated stress concentrations in graphite/epoxy composite plates containing a circular hole. The plates were subjected to unidirectional loading. The study was based on unidirectional laminates with oriented fibers, balanced symmetric angleply, crossply and [0 / ± β / 90]s laminates. The authors [17] used the approach of Lekhnitskii to evaluate the stress concentration in graphite/epoxy laminates of varying fiber orientation subjected to uniaxial tension. Some of the important details of their method are discussed below. 3
18 1.3.1 Stress Analysis According to classical lamination plate theory, the strain and resultant force per unit length relation in an orthotropic plate loaded in the plane of the plate is given by: A ' A ' A ' ε x N x A ' ' ' ε y = 1 A A 6 N y γ xy A ' A ' A ' N xy (1.3.1) where ' A ij is the elastic compliance matrix and is computed from the stiffness coefficient transformed into the x, y, z coordinate system of the individual lamiae by Q ij 1 ' n k ( A ) = A = Qij ( h h ) ij ij k= 1 k+ 1 k (1.3.) where h is the plate thickness. From the Lekhnitskii s theory of two dimensional anisotropic elasticity, the stress function F(x, y) satisfying the equilibrium and compatibility condition is the solution of the biharmonic equation ( ) ' F ' ' F ' F A + A + A + A = x x y y 4 (1.3.3) The laminates were loaded uniaxially (N x = p, N y = 0, N xy = 0) at an angle φ to the principal axis to the plate as shown in Fig and Fig The circumferential stress on the boundary of the hole is given by the expression ( n) ' A cos φ + µ µ sin φ µ µ cos φ σ θ = p A ' (1.3.4) θ + ( 1+ n) cos φ + µ µ sin φ sin φ n( 1+ n µ µ ) sinφ cosθ sinφ cosθ 1 1 4
19 where θ is the location around the hole measured from the principal axis of the plate and µ 1 and µ are roots of the characteristic equation In equation 1.3.4, the compliance ( ) 4 A ' ' ' ' 11µ + A A µ + A = 0 (1.3.5) 66 1 ' A θ in a direction tangent to the opening can be obtained from ( ) A ' A ' sin 4 θ A ' A ' sin θ cos θ A ' cos 4 θ θ = (1.3.6) The roots of the characteristic equation are related to the elastic compliance by A ' µ µ = (1.3.7) 1 A ' 11 A ' σ 11 µ µ cos φ 1 sin φ θ ' 1 A θ and = p + ( + n) (1.3.8) If the plate is loaded in a direction parallel to the principal axis of the plate, then φ = 0 and equation (1.3.4) becomes equation (1.3.9). A ' σ = p 11 µ µ cos φ ( 1 n) sin φ θ ' A θ (1.3.9) Equation (1.3.4) was used to evaluate the stress distribution for both unidirectional and crossply laminates as shown in Fig and Fig.1.3. respectively. From the curves in Fig it is observed that the maximum stress concentration is obtained where the fibers are aligned with the load direction. As the fiber angle changes, the magnitude of the stress concentration is reduced. Also, the location of the stress concentration varies with the fiber orientation. The results for crossply laminates were obtained by varying the loading direction relative to principal axis. 5
20 From Fig.1.3. it can be observed that as the load direction changes relative to the principal axis, the stress concentration is reduced. Fig Effect of fiber orientation on stress concentration in a unidirectional laminate [17]. Fig.1.3. Effect of loading direction on stress concentration in a crossply laminate [17]. The stress distribution for sym mmetric angleply [ ] s ± β and the [0 / ±β / 90 s laminates was evaluated by equation (1.3.9) which is shown in Fig and Fig respectively. From Fig it is observed that unlike unidirectional laminates the location of the maximum stress 6 ]
21 concentration for angle ply laminates didn t shift with the ply orientation. In angle ply laminates the maximum value of the stresss concentration was observed at a location 90 degrees relative to load axis. From Fig and Fig it can be observed that the maximum stress concentration decreases more rapidly for symmetric angle ply laminates than for unidirectional laminates with similar fiber orientation. Thus it can be observed that the angleply laminates reduce the maximum stress concentration. Fig Effect of ply orientation on stress concentration in angleply laminate [17]. 7
22 Fig Effect of fiber orientation of offaxis plies on stress concentration in laminates [17]. 0 / / 90 s n [ ±β ] Fig shows that changing orientation of the ± β plies influences the magnitude but not the location of the maximum stress maximum stress concentration concentration for [ β ] 0 / ± / 90 s laminates. The Location of the in these laminate was observed at 90 degrees to the loading direction. The Stress concentration was found to decrease as plies deviated from the loading direction. However, after approximately β =± 60 degrees, the maximum stress concentration ] again began to increase. For [00 / ± β / 90 s laminates, the offaxis ± β ply orientation within a range of 45 to 60 degrees generated the optimum design to reduce the stress concentration. This motivates the study of nontraditional 1 laminates for reducing the stress concentration and subsequently observing the effect of reduced stress concentration on the laminate strength. 1 Nontraditional laminates are the ones where β necessarily need not be 45 degrees. 0 and 90 degree can also be altered in such laminates. The name traditional laminates is given to the ones where the layup comprises of 0, 90 and 45 degrees. 8
23 1.4 Effect of stacking sequence on the strength Failure in composites can be decomposed into two modes; inplane failure and out of plane failure. The inplane failure which is the focus of this study is tensile in nature. Out of plane failure is usually referred to as delamination. The aim of this section is to understand the effect of the stacking sequence of plies on these two modes of failure Net tension strength Yan et al. [18] compared the response of notched composite laminates when subjected to open and filled hole tension. The authors considered the effect of ply orientation, lateral constraint and washer size in this study. T800/3900 graphite/epoxy prepreg was selected for the study and the laminates were divided into groups. Group 1 comprised of laminates A, B, C and D while Group included laminates E, F, G, H and I. Fig Comparison of nettension strength between open and filledhole laminates [18] 9
24 Fig provides a comparison between the groups regarding the open and filled hole tensile strength. The details of the stacking sequence of the two groups are provided in Table Table Stacking sequence of group 1 and group [18]. Laminates Stacking Sequence A [ ] 0 / 90 S GROUP 1 B [ 0 / 45 / 90 / 45] S C [ 0 / ± 45 / 90] S D [ ± 45 / 0 / 90] S E [ 45 / 0 / 0 / 45] S F [ 45 / 0 / 0 / 45 / 0 / 90] S GROUP G [ 45 / 0 / 0 / 45 / 0 / 90 / 0 / 90] S H [ 45 / 0 / 0 / 45 / 0 / 0 / 90] S I [ 45 / 0 / 0 / 45 / 0 / 0 / 90 / 0 / 0 / 90] S For group 1, no strength reduction was found for filledhole specimens compared to open hole specimens. For group the notch strength of filled hole laminates was lower than the openhole laminates. It was observed that the change in stacking sequence in the quasiisotropic configuration of [ 0 / ± 45 / 90] S had a small effect on the net tensile strength. Radiographic analysis of the two groups led to the conclusion that damage in group 1 was mostly confined near the stress concentration areas and propagated from the hole region toward the free edge. The damage was found to be in form of matrix cracks and fiber breakage. For group additional damage modes like delamination and fibermatrix splitting were found. Higher strength of group in net tension study is obvious due to presence of higher number of 0 0 plies. However, it seems 10
25 that a higher percentage of 0 degree plies also made the laminates of group prone to delamination and fibermatrix splitting Delamination strength. Delamination in laminated composites is a major cause of strength degradation. Interlaminar stresses generated near free edges are responsible for this mode of failure. Generally multidimensional laminates combining angleply and cross ply sub laminates, exhibit effects of both shear coupling and Poisson s ratio mismatch. Thus in the case of multidirectional laminates all three interlaminar stresses (σσ, τ, τ ) are present and the stacking sequence plays a major Z XZ YZ role in governing the nature of these stresses. Pipes et al. [18] tested three stacking sequences [ ± 15 / ± 45] s, [ ] 15 / ± 45 / 15 s an nd [ ] σz through the thickness is shown in Fig ± 45 / ± 15 s under a uniaxial tensile load. The distribution of Fig.1.4. Effect of stacking sequence on the through thickness distribution of nterlaminar stress σz near the free edge [18] It is evident that both the magnitude and sign of the stress can change drastically with stacking sequence. From a design point of view it seems that stacking sequences that result in minimum σzstresses should be considered. In the case of notched laminates the effect of interlaminar stresses is more detrimental. In this case, edge effects were accentuated by the stress concentration on the edge of the hole. Denial et al. [19] used two boron/ /epoxy panels of 11
26 0 / ± 45 / 0 s and 45 / 0 / ± 0 stacking sequence with a circular hole and subjected them to s axial tension. The overbar overr the 0 degree plies indicates that the laminates are symmetric about the mid plane of the ply. These two stacking sequences resulted in tensile and compressive interlaminar normal stress ( σ ) near the edge of the hole at the point of z maximum stress concentration. Fig shows the fringe pattern in a photoelastic coating around the hole near failure. 0 / ± 45 / 0 45 / 0 ± / 0 s s Fig Isochromatic fringe patterns in photoelastic coating around the hole in boron/epoxy specimenss of two different stacking sequences [19] The pattern for the 0 / ± 45 / 0 specimen is fairly symmetric with s a lower stress concentration. The pattern for the ± 45 / 0 / 0 specimen skewed with the higher stress s concentration. The failure surface of the two specimens is also very different as is shown in Fig
27 ±45 / 0 / 0 0 / ± 45 / 0 s s Fig Failure patterns of boron/epoxy tensile panels with holes of two different stacking sequences [19]. The ± 45 / 0 / 0 specimen failed horizontally in catastrophic manner at an s average applied axial stress of 61.7 Ksi. The 0 / ± 45 / 0 specimen failed by vertical cracking in a non s catastrophic manner at an applied stress of 76.4 Ksi. The specimen then split into two strips that carried a much higher ultimate stress of 105 Ksi. Park H.J. [0] used finite element analysis to study the effects of stacking sequence and clamping force on delamination bearing strength of mechanical fastened joints in carbon/epoxy composite laminates. 3D contact stress analysis was performed to mimic the bolthole interaction. His FEA procedure was based on a layer wise theory along with the Yedelamination criterion. The problem was stu sequence of [ ] 90 / 0 S was more udied for [ 0 / 90] S &[ ] e advantageous than [ ] 90 / 0 S layup. Park found that a stacking 0 / 90 S from the aspect of delamination 13
28 strength. Similar conclusions were obtained by [1,, 3] with experimental and finite element analysis. Park [4] also investigated the effect of stacking sequence and clamping force on notched composites using an Acoustic Emission (AE) technique. The effect of stacking sequence on the ultimate and the delamination strength in bolted and pinned joints was compared. The results for both joints were quite similar. The study was based on a stacking sequence of quasiisotropic layups[ 903 / 453 / 03] S ±, [ ] 903 / 03 / 453 S ± and[ 03 / ± 453 / 90] S. The results indicated that layup [ ± ] had the highest bearing strength and the layup [ ] 903 / 453 / 03 S 903 / 03 / 453 S the second highest one. The layup [ ] 903 / 03 / 453 S the stacking sequence [ ] 903 / 03 / 453 S ± had ± had the highest delamination strength. Thus ± which had the highest delamination strength and second highest ultimate bearing strength should be preferred from the view point of its characteristics of failsafe delamination failure. The 90 degree layers have been found to play a very important role in the bearing strength of composite laminates. Composite laminates with 90 degree layers on the surface have higher delamination strength than the laminates with 90 degree plies in the center. Kaminski B.E. [5] has reported similar findings using [0/90] glass/epoxy coupons. He found with low scatter that the coupons with 90 degree layers on the surface were 9% stronger than the ones with 0 degree layers on the surface. 1.5 Failure Criteria study Failure criteria for homogenous isotropic materials, such as the maximum normal stress (Rankine), maximum shear stress (Tresca) and maximum distortional energy (Von Mises) are well established. Macromechanical failure theories for composites have been proposed by extending and adapting isotropic failure theories to account for anisotropy in the stiffness and strength of the composites [3]. Lamina failure theories can be broadly classified into mode based and interactive. 14
29 Mode based Theories such as maximum stress, maximum strain, HashinRothem in which specific failure modes are predicted by comparing individual lamina stress or strains with corresponding strength and ultimate strains are mode based or noninteractive failure theories. The maximum strain theory does allow for some interaction of stress components due to Poisson s effect [3] but is still considered a mode based theory. Jenkins [6] in 190 was the first to use an extension of the maximum normal stress theory or Rankine theory for orthotropic laminae. Kelly [7] used the maximum stress theory in 1966 to predict the off axis strength of unidirectional composites as a function of fiber orientation by three different curves corresponding to 3 different failure modes. According to the maximum stress theory, failure occurs when at least one stress component along one of the principal material axes exceeds the corresponding strength in that direction. For a three dimensional state of stress with transverse isotropy on the 3 plane the following set of inequalities must be satisfied to avoid failure S 1C < σ 1 < S 1T S C < σ < S T S 3C < σ 3 < S 3T S 1C < σ 1 < S 1T S 3C < σ 3 < S 3T S 13C < σ 13 < S 13T. (1.5.1) In the above equations S i (for i = 1,, 3) denotes the ultimate value of stress in the principal normal directions and S ij (for ij= 1, 3 and 13) stands for ultimate shear value in the principal shear directions. C and T are used to distinguish between the strength parameters in compression and tension respectively. 15
30 In 1967 Waddoups [8] proposed the Maximum Strain Criterion for orthotropic laminae as an extension of the Maximum Normal Strain Theory (or Saint Venant s Theory) for isotropic materials as ε 1C < ε 1 < ε 1T ε C < ε < ε T ε 3C < ε 3 < ε 3T ε 1C < ε 1 < ε 1T ε 3C < ε 3 < ε 3T ε 13C < ε 13 < ε 13T (1.5.) Hashin and Rotem found that failure of a lamina under a general inplane loading can be characterized by two failure criteria, one for fiber failure and the other for inter fiber failure [9] as σ 1 = S ors 1T 1C 1 σ σ 1 + = 1 STorSC S1 (1.5.3) (1.5.4) These criteria can be extended for a general threedimensional state of stress in terms of stresses acting on the three principal material planes and related to the expected failure modes on those planes. σ 1 = S ors 1T 1C σ σ 3 σ = 1 STorSC S3 S1 1 (1.5.5) (1.5.6) σ 3 σ 3 σ = 1 S3 TorS3C S3 S13 (1.5.7) The strength parameters used in the equations should be based on the sign of the stresses. That 16
31 means if the stress in the longitudinal or 1direction is tensile (+) then the limiting strength should be tensile and for compressive stress () the strength parameter should be compressive. This holds true for transverse and shear stresses as well. In the criteria above, the strength values are the ultimate values when the stressstrain behavior is linear to failure. In case of nonlinear behavior, the strength values can be defined as proportional limits of the corresponding stressstrain curves. Hashin proposed a modification of HashinRotem theory. He proposed more interactive criteria for tensile failure of the fiber and for combined transverse compression and shear. In the latter case he introduced the effect of transverse shear strength in the criterion Quadratic Failure Theories The quadratic failure criteria are interactive and based on curve fitting considerations and not on physical failure modes [30]. The stress terms are included in one expression and failure is predicted without reference to particular failure mode. The deviatoric and distortional energy has been proposed by many investigators (e.g. Von Mises, Hencky, Nadai) in various forms as a failure criterion for isotropic ductile metals. For a twodimensional state of stress in the principal stress directions, the von Mises yield criterion has the following form [3] ( σ ) ( σ ) σσ ( σ ) + = (1.5.8) 1 1 yp Hill modified this criterion for case of ductile metals with anisotropy and proposed the following form. Aσ + Bσ + Cσσ + Dσ = (1.5.9) For inplane and out of plane shear stress the sign of limiting stress is immaterial as the value of shear in tension and compression is same. Also for the current work S 1 = S 3 = S
32 where A, B, C, D are material parameters characteristic of the current state of anisotropy. The modified form of the criterion led to TsaiHill criterion which in three dimensional form can be written as [31] σ 1 σ σ S ors S ors S ors 1T 1C T C 3T 3C ( S ) or( S ) ( S ) or( S ) ( S ) or( S ) 1T 1C T C 3T 3C ( S ) or( S ) ( S ) or( S ) ( S ) or( S ) T C 3T 3C 3T 3C σσ 1 σ σ σ 3σ 1 ( S3 T ) or( S3C ) ( S1 T ) or( S1 C ) ( ST ) or( SC ) σ σ σ S1 S3 S13 1 (1.5.10) Failure is predicted by this theory when the left side of the equation is greater than or equal to one. The theory is similar to HashinRotem theory in the sense that it also takes into account the sign of the stresses in the principal material direction. However unlike HashinRotem theory it fails to provide information regarding the mode of failure. The quadratic nature of the theory has been criticized because it is based on Hill s theory, which is suitable for homogenous, anisotropic and ductile metals, whereas most composites are strongly heterogeneous and brittle. One more problem with the Hill s theory is that it predicts that failure will never occur in hydrostatic state of stress (σ 1 = σ = σ 3, σ 1 = σ 3 = σ 13 =0). Due to shear coupling in composites, however, a hydrostatic state of stress can produce shear strains and failure. Hoffman s equation due to its linear terms, could predict failure for a hydrostatic state of stress. The three dimensional form of the Hoffman equation is given as. 18
33 S S S S S S S S S S S S ( σ σ ) ( σ σ ) 1 3 1T 1C T C 3T 3C T C 3T 3C 1T 1C ( σ 3 σ1) + σ1+ σ S3 T S3C S1 T S1 C ST SC S1 T S1 C ST SC 1 1 σ 1 σ 3 σ 13 σ S3 T S3C S1 S3 S13 (1.5.11) However, all of the quadratic theories form special case of a more general quadratic interaction criterion. In 1971 Tsai and Wu [3] proposed an improved and simplified version of a tensor polynomial failure theory for anisotropic materials originally proposed by Gol denblat and Kopnov [33]. The proposed criterion in contracted notation can be written as Fσ + Fσσ = 1 (1.5.1) i i ij i j where contracted notation i, j = 1,,.., 6. F i and F ij are experimentally determined strength tensors of second and forth rank, respectively. In order to avoid failure, the left hand side of the equation (1.5.1) should be less than one. The details of finding the coefficients of the stress terms are in [34]. The three dimensional form of the TsaiWu criterion which is used for current work is given as σ σ σ S S S S S S S S S S S S σσ σ σ σσ 1 3 σ1+ σ + σ T 1C T C 3T 3C 1T 1C T C 3T 3C S S S S S S S S S S S S 1T 1C T C T C 3T 3C 1T 1C 3T 3C σ σ σ S1 S3 S13 1 (1.5.13) Farsakh et al. [35] proposed an energy based failure criterion for nonlinear composite materials which was included as a part of the current work. The three dimensional form of the criterion in contracted notation can be written as 19
34 ~ U U i ij Ui = + = 1 U im U (1.5.14) ijm Where i, j = 1,, 3 and U i, U ij correspond to extensional and shear strain energy densities respectively. According to the energy criterion, failure can be avoided if the left hand of equation is less than 1. The strain energy densities can be found as U U 1 = σε 1 = σ ε i i i ij ij ij. (1.5.15) The subscript m denotes the corresponding maximum value of strain energy density. The stress and strain terms in equation (1.5.15) can be replaced with the maximum strength and strain values for finding values of denominators of equation (1.5.14). 1.6 Applicability of Laminate Failure Theories The validity and applicability of any failure theory depends on its agreement with experimental results. Recently two main efforts were aimed at evaluation of laminate failure theories. One of them was by Sun [36, 37] and the other by Hinton et al. [38]. Sun [36, 37] reviewed six failure theories and compared theoretical predictions of the laminate strength with experimental results for six composite materials and various loading conditions. He found that for fiber dominated laminates the maximum strain, maximum stress and Hashin Rotem gave the best predictions. The interactive theories gave good predictions for matrix dominated strength. Hinton et al. [38] conducted a World Wide Failure Exercise (WWFE) over a twelve year period for the purpose of assessing the predictive capabilities of some of the most prominent failure theories of composite materials. The exercise covered nineteen theories, four composite material systems, six laminate configurations and four loading conditions. The leading theories (Tsai, Puck, Zinoviev, Bogetti, Cuntze) were compared. One observation of this exercise 0
35 was that even for unidirectional lamina, predictions of these theories differed by up to % from each other. The authors also found that these theories tended to underperform in situations where shear and matrix behavior plays a significant role in the failure process and where large deformations were present before final failure occurred in the experiment. One of the findings of the literature concerning failure criteria was that the theories that perform well for a certain set of material properties and under given loading condition may not do well if these variables are changed. This makes the task of generalizing the applicability of failure theories extremely difficult. The best practice is to compare the theoretical predictions with accurate and reliable experimental results. In the current work the strength predictions of seven prominent failure theories were compared with experimental data to check their accuracy in predicting the First Ply Failure strength for notched composite laminates under tensile loading condition. 1.7 FEA Study A study of some of the established FEA methodologies was carried out to compare their advantages and disadvantages which would assist in the selection of a method most suitable for the current work. Tay et al. [39] presented a new FEA based approach known as the element failure method (EFM) which they claimed to be better than the traditional material property degradation method (MPDM) and the fracture mechanics approach. In the MPDM, the value of certain material properties in the constitutive relation is reduced when damage or failure is determined e.g. if failure is determined to have occurred in the fiber direction (as in the breaking of fibers in tension), the fiber direction Young s modulus (E 11 ) may be set to zero. This is a special case of MPDM and is called the Ply Discount Method. Normally in the published literature the authors set the degraded material properties to a small percentage of the original. This is done to avoid the stiffness matrix of the FEA model from becoming illconditioned which 1
36 is turn stops the FEA code from converging. MPDM has another major drawback. There is uncertainty regarding the property that should be degraded e.g. if transverse cracking or failure is predicted in a composite it is not clear if only the transverse Young s Modulus E or both this and the inplane Shear Modulus G 1 should be reduced. Additionally, the effect of damage on the Poisson s Ratio ν 1 and ν 1 is not obvious or easily determined. Fracture mechanics has been applied to composites although some have cited some major drawbacks in the traditional approach. First of all in composites it is not easy to clearly identify and define cracks and crack tips as is done with metals. In some exceptional situations a crack may be defined such as in the case of a single delamination in a laboratory fracture test specimen. However, even in such situations, mechanisms such as fiber bridging across crack surfaces, delamination kinking, or branching into other fracture planes greatly complicates the analysis and can lead to wrong results. The EFM modifies nodal forces to reflect changes in the stress bearing capability of the damaged material. The stiffness matrix remains untouched and drawbacks of MPDM are automatically avoided. The EFM along with the Strain Invariant Failure Theory (SIFT) have been recently proposed by Gosse [40]. An in house D FE code was used to implement the methodology. A three point bend test was used as test problem for damage prediction. EFM based approach was very attractive for predicting damage in composites. However the drawback of using EFM based approach for this thesis was the complexity to successfully incorporate it in commercially available software like ANSYS TM, which was used for the numerical work of this study. Wang et al. [41] used both; linear elastic and a progressive damage approach to predict the strength of unnotched and notched quasiisotropic laminates. AS4/ material was used and laminates were subjected to tension and compression tests. It was found that the linear elastic approach underestimated the First Ply Failure strength (FPF) or overestimated the Last Ply
37 Failure (LPF) strength for unnotched laminates. The progressive damage was able to predict the unnotched strength, provided that the nonlinear shear behavior was accounted for and the appropriate failure criterion was used. They used ABACUS FEA software and shell elements to implement material degradation. For the purpose of comparison, a characteristic distance approach was applied to the openhole strength problem. In this approach the authors had to calibrate the model for tension and compression loading and for a particular hole size. Although they found that no consistent relationship existed between the characteristic distance and the hole size for the tension case, the compression characteristic distance was related to the hole diameter by the following relation where d 0 was the characteristic distance and d was the hole diameter. d 0 = * d (1.7.1) The predicted accuracy of the tensile test appeared satisfactory with a maximum discrepancy of %. However, the prediction of the compression test was less accurate with a maximum error of 15%. Thus this approach does not appear to be very robust. 1.8 Conclusion The literature review pointed to the fact that stress concentration in composites with a circular hole is a function of the fiber angles. For traditional laminates [ β ] orientation 0 / ± / 90 s the off axis ± β has been found to generate an optimum design for reducing stress concentration where 45 β 60. Further, the effect of stacking sequence on the failure modes in laminates is quite evident. For multidirectional laminates which show shear coupling and Poisson s mismatch, interlaminar stresses are present and thus a particular stacking sequence can be generated for resisting delamination growth. Seven failure theories (MaxStrain, MaxStress, HashinRothem, TsaiWu, TsaiHill, Hoffman and energy) were presented and would be applied 3
38 along with an appropriate FE method. Although some have proposed damage based FE models for strength prediction of laminated composites, but for the current study a linear elastic approach was chosen in order to determine the first ply failure (FPF).. 4
39 . 3D FEA MODEL.1 Introduction The literature review behind the current study provided a motivation to find the effect of tailoring fiber orientation and stacking sequence on the openhole tension (OHT) strength of the laminates. This chapter aimed at introducing a 3D FE model that could show the through thickness strain field and the sensitivity of stress concentrations to the fiber orientation and stacking sequence of a laminated composite. A standard quasiisotropic layup ( ) 45 / 90 / 45 / 0 s was used as baseline and compared with other nontraditional layups. Fig...1 Geometry of the laminated plate along with the model geometry 5
40 .. Laminate Geometry The laminate geometry under consideration is shown in the Fig...1. The composite plate was 1 inches in height, 1.5 inches in width and 0.07 inches in thickness with a 0.5 inch hole drilled in the center. The effect of the stress concentration due to the presence of circular notches diminishes at a distance of 9 radii from the edge of the hole [4]. Keeping this in mind, the height of the FE model was restricted to 1.5 inches i.e. ten times the radii of the hole. The model geometry shown in Fig...1 is one eighth of the original plate..3 Material Properties The properties of T600:1533 carbon/epoxy material were found using inplane tests of five specimens of [0] 6, [90] 16 and ( ± 45) 3 s laminates. The 0 and 90 degree coupons were used to determine the inplane ultimate tensile strength in longitudinal and transverse direction respectively. Due to a linear relationship between stress and strain in unidirectional (i.e. 0 and 90 degree) laminates, the ultimate stress and strain is equivalent to the yield stress and strain. However, the inplane shear behavior is nonlinear. For the nonlinear shear behavior, the yield strength should be used in order to determine the First Ply Failure of a laminate [3]. To determine this yield point, two methodologies were considered. One is the double notch shear test and other is the cyclic loading and unloading of ± 45 degree coupons. The double notch shear test was found unsuitable for finding inplane shear properties as described in detail in section.6. The uniaxial loading of a ± 45 degree coupon can be used to find out the inplane shear stress and shear strain. Using the stress transformation relation [34] and referring to Fig we get σ 1 σ = τ [ T ] D 1 σ x σ y τ xy (.3.1) 6
41 where T D is a two dimensional transformation matrix given by [ T ] D cos sin cos sin = sin cos cos sin cos sin cos sin cos sin ( θ) ( θ) ( θ) ( θ) ( θ) ( θ) ( θ) ( θ) ( θ) ( θ) ( θ) ( θ) ( θ) ( θ). (.3.) For uniaxial loading condition ( σ τ 0 ± 45 y = xy = ) of ( ) 3 laminate, s σ τ x 1 = (.3.3) Using the transformation relation for strain we get ε1 ε x ε = [ T D] ε y, (.3.4) γ1 γ xy and solving for shear strain in the principal material direction we obtain γ = ε + ε. (.3.5) 1 x y ± 45 The stressstrain curve obtained by the repeated loading and unloading of ( ) 3 is shown in Fig The ± 45 degree coupons were loaded in steps, starting from 3651 Psi to Psi. The material yielded well within a tensile stress of Psi. Hence, further increase in load was not necessary. At the end of each load step, the test was stopped and the load was allowed to drop to the initial value (approx. 34 lbs). The load was held at this stage and one of the grips holding the coupons was relaxed. The spike marked by O in Fig..3.1 indicates this sudden release of grip. This relaxation in the load allowed for viscoelastic strain recovery. This is s 7
42 marked by V in Fig The time dependent recovery strain is shown in appendix A1. Unlike metals, the 0.% strain rule may provide misleading results for polymers. Few steps were followed to come up with a yield stress and corresponding yield strain suitable for this study. Firstly, damage induced in the material due to each loading cycle was found by plotting the recovered viscoelastic shear strain after each stress cycle with the shear stress. One of the recovered shear strain points is denoted as V P in Fig Ten such points could be extracted from Fig..3.1 and were plotted with respect to their corresponding shear stress values. This is shown in Fig Shear Stress (τ 1 ), (Psi) V P O ShearStress (τ 1 ) V Shear Strain (γ 1 ),(in/in) ± 45 Fig..3.1 Shear Stress Vs Shear Strain curve for cyclic loading and unloading of ( ) 3 laminate. s 8
43 Viscoelastically Recovered Shear Strain, (in/in) τ 1 =4381Psi Shear Stress (τ 1 ), Psi Fig..3. Viscoelastically recovered Shear Strain Vs Shear Stress 6000 Shear Stress (τ 1 ), (Psi) A(6941, 4381) ShearStress (τ 1 ) Shear Strain (γ 1 ),(in/in) Fig..3.3 Shear Stress Vs Shear Strain for defining Yield Stress From Fig..3. it can be seen that up till the shear stress of 4381 Psi, the strain recovered completely. However, during the third repetitive load cycle there was some damage in the material. Thus the maximum shear stress corresponding to the third repetitive loading cycle can be assumed as the yield shear stress in the material. It is denoted by the Y axis value of point A in Fig Fig..3.3 is same as Fig..3.1 except that it shows only the first three stress cycles. The X axis value of point A in Fig..3.3 denotes the yield shear strain of the composite material. 9
44 The properties from the inplane tests and from Fig..3.3 were used to define the tensile orthotropic behavior of each lamina. From [55] we could assume that S13 = S assumption didn t affect the results as during FEA it was observed that out of plane stresses were 3. Further, this smaller (10 times) as compared to inplane stresses. The compression properties were obtained from [43]. 3 Table.3.1 Material Properties of T600:1533 carbon/epoxy. 6 6 E 1= E = E 3= E 6 G 1 = G13 = G E 1 G 3 = 1+υ υ 1 = 0.98 S 1T = S 1 = C 3 3 υ 3= 0.35 υ13 = υ1 3 S T = S3 C = S C S3 T = S T 3 3 S C = S C = S C S 1 = , S = S = S, 3 ( ) Model Formulation Fig Geometry used for the FEA study. 3 Modulus and strength properties are in Psi. 30
45 The numerical simulation was carried out using the ANSYS TM 10.0 FEA package. A static tensile pressure P was applied on the top face of the model in the Y direction as shown in Fig The model geometry used 3 symmetric boundary conditions (BCs) on three mutually perpendicular planes. The front view in Fig..4.1 shows symmetric B.C. applied to the faces resting on the XZ and the YZ reference plane. Thus the new width was half the original width of the plate i.e. W/. The height was reduced to 10 R, R being the radius of the hole. The reason for choosing this height has been explained in section.. Since the laminates were symmetric through the thickness, so the model thickness was reduced to half i.e. Thk/. Thus, effectively, oneeighth section of the actual plate was used for the FEA. Fig..4. Individual volumes representing each lamina through the thickness A one eighth model meant that only 8 plies needed to be created instead of 16 as shown in Fig..4.. Each of the plies in the laminate geometry was represented by a single volume layer. The ANSYS TM material model interface allows the stiffness matrix input to represent each lamina. The coefficients of the stiffness matrix are a function of fiber orientation. Since the model 31
46 geometry was in the global coordinate system (C.S.), represented by the XYZ reference frame, the stiffness matrix for each lamina was transformed from the principal material to the global C.S. by the following relations [3]. [ σ] [ ][ σ] T 1,,3 3 D x, y, z = (.4.1) Or 1 [ σ] [ ] [ σ] =, (.4.) T x, y, z 3 D 1,,3 where [ σ ] x, y, z and [ σ] 1,,3 are the contracted 3D stress matrices in the global (X, Y, Z) and the principal material (1,, 3) C.S. respectively. [ T3D] represents the three dimensional form of the coordinate transformation matrix given by [ ] T3 D ( θ) ( θ) ( θ) ( θ) ( θ) ( θ) ( θ) ( θ) cos sin cos sin sin cos cos sin = cos( θ) sin( θ) sin( θ) cos( θ) 0 cos( θ) sin( θ) cos( θ) sin( θ) cos ( θ) sin ( θ) (.4.3) From Hooke s law [ σ] [ Q] [ ε] =, (.4.4) 1,,3 1,,3 1,,3 where [ Q] 1,,3 is the contracted form of 3D stiffness matrix in the principal material C.S. and can be expressed in terms of the material properties of Table.3.1 as 3
47 [ Q] 1 υ 1 υ E1 E1 E1 υ 1 1 υ E1 E E υ 13 υ E E E G G G 1 3 = 1,, (.4.5) By substituting the value of [ σ] 1,,3 from equation (.4.4) into equation (.4.), we get and replacing [ ε] 1,,3 by [ D][ ] T ε we obtain 3 x, y, z 1 [ σ] [ ] [ ] [ ε] = T Q (.4.6) x y z,, 3D 1,,3 1,,3 [ σ] [ T ] 1 [ Q] [ T ][ ε] = (.4.7) x, y, z 3D 1,,3 3D x, y, z Equation (.4.7) can also be written as [ σ] [ Q] [ ε] =, (.4.8) x, y, z x, y, z x, y, z where [ Q] [ T ] 1 [ Q] [ T ] = (.4.9) x, y, z 3D 1,,3 3D [ Q] x, y, z was used as stiffness matrix in the FE model. Solid 64 brick element was used for this work. The element shown in Fig..4.3 is defined by eight nodes having 3 degrees of freedom (D.O.F) at each node in the form of translations in the nodal x, y, z direction. The element has large deflection capabilities. The element coordinate system was set parallel to the global xyz 33
48 coordinates using the setting Keyopt (1)=0 as shown in the AppendixA. Then using equation (.4.9) the orientation of the elements in each lamina was defined. Fig Solid 64 element used for the FE model (a) (b) Fig..4.4 (a) Preliminary mesh of Baseline laminate with 307 elements (b) Refined mesh of Baseline laminate with 5596 elements P P B B A A Fig..4.5 Comparison of longitudinal direction (y) strain contours for meshes (a) and (b) of Fig Stress P is acting along y direction. 34
49 The mesh refinement of the model was carried out in two stages. In the first stage, elements were increased in the XY plane of the laminate. The preliminary mesh as shown in Fig..4.4 (a) had only 307 elements. Progressive refinement was carried out until convergence was achieved and the final mesh had 5596 elements. The convergence study was carried out at two points, A and B on the surface of the laminate as shown in Fig A static tensile stress of 30,000 Psi was applied throughout the convergence study. Longitudinal direction strain (ε y ) was used for checking convergence ε ya, in/in ε yb, in/in Number of Elements Number of Elements Fig..4.6 Variation of longitudinal direction strain at point A ( ε ya ) with increase in number of elements Fig..4.7 Variation of longitudinal direction strain at point B ( ε yb ) with increase in number of elements Fig..4.6 and Fig..4.7 show the variation in the longitudinal direction strain ( ε y ) at point A and B respectively with mesh refinement. After 5596 elements, further refinement didn t seem to have any effect on the strain values. 35
50 (a) (b) Fig (a) Through thickness mesh with one element per ply. (b) Mesh with two elements per ply. In the next stage, elements through the thickness were refined. Instead of one element per ply (Fig..4.8 (a)), two elements per ply were used (Fig..4.8 (b)). The result of increasing the elements in thickness direction is evident from Fig..4.9 (a) and Fig..4.9 (b), with elements per ply mesh giving a better strain contour. The term better is qualitative in nature. Strain contours with a two elements per ply mesh were much smoother and thus meant reduced error estimation. Further refinement with 3 elements per ply was not possible as the aspect ratio 4 of the elements was too large and so no mesh was generated. The final refinement thus comprised of elements. 4 Aspect ratio of an element in FE model is the ratio of the longest and the shortest side of the element. Typically this ratio should be between to 4. 36
51 (a) (b) Fig..4.9 (a) Longitudinal direction strain contour of Baseline laminate for mesh with one element per ply (b) Longitudinal direction strain contour of Baseline laminate for mesh with elements per ply..5 Model Validation. The material properties of Aluminum 7075 from Table.5.1 were used in the 3D FE model. The strain concentration factors (K t ) from the FEA study were compared with the analytical results [43] for different hole diameter (d) to width (w) ratios. Table.5.1 Material properties of Aluminum 7075 [43] 6 E = Psi υ = 0.33 E G= (1 + υ) P N B A Fig..5.1 Longitudinal direction strain ( ε y ) contour of 3D model having Aluminum 7075 properties 37
52 Fig..5.1 shows the contours of the longitudinal direction strain, when the 3D model with isotropic properties from Table.5.1 was subjected to a tensile stress (P) of 30,000 Psi. This corresponded to a load of 3150 lbs over an area of square inches. The edge of the hole marked as A experienced a maximum longitudinal strain of while B had a minimum value of The symbol N is an approximate nominal strain location ε YA, (in/in) ε YN, (in/in) Through thickness at A, (in) Through thickness at N, (in) (a) (b) Fig..5. (a) Through the thickness variation of longitudinal direction strain at location A (ε YA ). (b) Through the thickness variation of longitudinal direction strain at location N (ε YN ). Fig..5. (a) and (b) show the variation in the longitudinal direction strain through the thickness of the model at locations A and N respectively. Since the model is symmetric through the thickness so the results have been plotted for half the thickness i.e inch. From Fig..5. (a) we concluded that although the strain change through the thickness of the hole was small but unlike Fig..5. (b) it was not constant. Theoretically, the stress concentration factor can be defined as K t σmax σnom = (.5.1) 38
53 where σ max is the stress near the point of highest stress concentration. In the Fig..5.1 this point is represented by A. σnom is to the nominal value of the stress and corresponds to the value of the stress in a plate without hole. Theoretically, nominal stress can be obtained as nom P σ = (.5.) A net and Anet = Agross A hole (.5.3) However, there is no way to get the stress or strain for the net area directly in Ansys. In Ansys the nominal stress is σ P FEA, nom = (.5.4) Agross For this study σ FEA, nom is selected from the region marked N in Fig This region approximately describes the stress state that is unaffected by the presence of hole. However, after applying correction factor K t can be found as σmax Anet εmax A k net t = = (.5.5) σ FEA, nom Agross ε FEA Agross For a D model, equation.5.5 can be applied to find the k t. However, from Fig..5. (a) it is evident that for a 3D model the strain through the thickness is not constant and an average of strain should be taken for finding maximum strain ( ε max ). Fig..5.3 shows the variation of longitudinal and transverse direction strains through the thickness of baseline laminate when subjected to a tensile stress of Ksi (4% baseline UTS). It supports the argument of using average strain through the thickness of the laminate near the point A (Fig..5.1). From both Fig..5. (b) and Fig..5.3 it is observed that the nominal strain values from the FEA models remain almost constant throughout the thickness. But it is still advised to use the average of all the strain 39
54 values through the thickness near the region where nominal strain values are assumed (point N in Fig..5.1). Point B, which also lies on the hole experiences minimum strain concentration Strain, (in/in) Through thickness distance, (in) εya εyn εxb Fig..5.3 Variation of longitudinal and transverse direction strain of baseline laminate through the thickness Thus the strain concentration factor (K t ) for the 3D model can be defined as K t εavg.max = Anet (.5.6) εavg. nom Agross which can be further simplified as K t εavg.max ( W d) = (.5.7) ε W avg. nom where ε avg.max and ε avg. nom are the average of the longitudinal direction strain values through the thickness of laminate at locations A and N (Fig..5.1) respectively. W and d are the width of the plate and the diameter of the hole respectively. 40
55 Strain Concentration Factor (Kt) Analytical 3D FEM d/w,(in/in) Fig..5.4 Strain concentration factor Vs hole diameter to width (d/w) ratio for Aluminum From Fig..5.4 it is clear that the strain concentration values from the 3D model closely follow those of the text book for isotropic material properties [43]. Another way of validating the 3D model is by comparing it with analytical solutions. Arjyal et al. [44] derived an expression for longitudinal direction stress ( σ ) as a function of distance from the edge of the hole along x direction. The stress distribution is given as y ( β ) ( β ) σ y ( ) 1 1 ( β ) ( ) ( β ) ( ) P 1 β1x βx x = P + FWC β 1+ β 1 β 1 r 1 1 x r β + r + x r (.5.8) where β β α β + α = + (.5.9) β β α β + α = + (.5.10) E x α 0 = (.5.11) Ey 41
56 Ex β0= υxy (.5.1) G xy E, E, υ, G x y xy xy are obtained from classical lamination plate theory. In equation (.5.8) the term FWC or finite width correction factor is a scale factor used to multiply the infinite plate solution for a notched plate to obtain the corresponding finite width plate solution. Tan [45] derived an expression for FWC applicable to the orthotropic plate solution r r r W FWC= 1 ( KT 3 + ) W W where r and W are the radius of the hole and the width of the plate respectively. 1, (.5.13) and 1 A11 A A1 K 1 T = + A11 A A1 + µ A66 A66, (.5.14) where K T is the stress concentration at the opening edge on the axis normal to the applied load for an infinite plate. Aij for i, j= 1,,6 are the effective laminate inplane stiffnesses with 1 and parallel and transverse to the loading direction, respectively. µ is defined as the ratio of the small axis over the large axis of an elliptical hole and therefore µ =1 for a circular hole. The stress distribution from equation (.5.8) can be easily converted into a strain distribution by σ y ε y = (.5.15) E y 4
57 P D FEA Analytical ε y, (in/in) Y x Distance from hole along x (in) Fig..5.5 Comparison of longitudinal direction strain distribution between 3D FE model and analytical solution for stress state around the hole for baseline laminate Fig..5.5 shows the comparison between the longitudinal direction strain distribution of the 3D 45/ 90 / 45/ 0 FE and analytical model along the X direction. The Baseline layup of ( ) was subjected to a tensile load of 7000 lbs for this comparison. The comparison between the 3D and analytical model indicated that the linear elastic model had the ability to accurately predict the strain profile in the vicinity of the hole. s 43
58 .6 Double notch shear test Ht P P S H S N H S L N Ht Y X Y Z S Uy=0 D Uz=0 W T 0.5W T (a) (b) Fig..6.1 (a) Geometry of double notch coupon (b) FE model geometry of double notch coupon Validation of the 3D FE model encouraged its use to determine the feasibility of a double notch shear test for estimating the inplane yield strength of T600:1533 material. The Double notch shear test was originally devised to find the interlaminar shear strength. However, for most cases the shears stress in principal material directions is assumed to be identical i.e. τ1 = τ13 = τ 3. The laminate fabricated for this test comprised of 38 zero degree laminae with the fiber axis aligned with y direction (Fig..6.1). The specimen as shown in Fig..6.1 (a) was 7.5 inches in height (H+ H t ), inches in width (W) and inches in thickness (T). H t denotes the part of the coupon covered with tabbing. This portion of the coupon is held by the grips of the MTS 44
59 tensile test machine. Two grooves ran parallel to each other throughout the width of the sample. The notches were inches in depth (D) and 0.16 inches in width (N). The gauge length (L) between the two notches was 0.55 inches. D and T are related by D > T/ (.6.1) Equation (.6.1) ensured that the gauge region remained under pure shear effect when the coupon was subjected to a tensile load. The FE model geometry is shown in Fig..6.1 (b). Owing to symmetry along the YZ plane, only half width of the sample was modeled. The height of the FE model geometry was restricted to 4.07 inches which is denoted by H in Fig..6.1 (a). The other boundary conditions used for restricting the rigid body motion and to simulate the effect of grips are given by U y x= 0, y= 0, z= T / = 0 x= 0.5 W, y= 0, z= T / (.6.) U z x= 0, y= 0, z= T = 0 x= 0, y= H, z= T (.6.3) 45
60 A B (a) (b) Fig..6. (a) FE mesh of the double notch test specimen (b) Interlaminar shear strain ( ) ε 13 contours of the double notch test specimen. The model was subjected to a static tensile stress (P) of Psi as shown in Fig..6.1 (b). Fig..6. (a) shows the mesh of the FE model geometry. The two arrows point to the zoomed in image of the A and B regions. As per equation (.6.1) the depth (D) of the notches exceeded the line of symmetry by inches through the thickness creating a gauge region. The FE model divided this gauge region into 3 laminae. That meant that shear could occur along four paths depending where the shear strain was maximum. These four paths have been numbered as 1,, 3 and 4 in the zoomed in image in Fig..6. (a). Fig..6. (b) shows the contours of the interlaminar shear strain( ε13) in the gauge area. Fig..6.3 shows the change in the interlaminar 46
61 shear strain ( ε13) along the nodes on the four paths. The nodes that formed these four paths were located on the surface of the gauge area. Although there is a small decrease in strain values from path 1 to path 4 but the general trend is same. The strain field in the gauge area is nonuniform with a relatively high strain concentration at the two notch ends. ε 13, (in/in) Distance from A, (in) ε13 path 1 ε13 path ε13 path 3 ε13 path 4 Fig..6.3 Variation of interlaminar shear strain ( ε 13) along the gauge length (L) from A to B ε 3, (in/in) Distance from A, (in) ε3 Path 1 ε3 Path ε3 Path 3 ε3 Path 4 Fig..6.4 Variation of interlaminar normal strain ( ε 3) along the gauge length (L) from A to B 47
62 From Fig..6.3 it is clear that the tensile loading condition created only little shear in the middle of the gauge region. From Fig..6.4 it is observed that the interlaminar normal strain is tensile at the ends and compressive in the middle. This showed that the failure in the gauge region is likely to initiate near the notches due to both shear and normal forces and not pure shear alone. Shokrieh et al. [46] reported similar results by using a double notched coupon of 90 degree laminae. For inducing pure interlaminar shear in the gauge area, Shokrieh et al. [46] performed a FEA study to find out the influence of notch size, gauge length and coupon thickness on the interlaminar shear response of the coupon and also to come up with a geometry that best suited shear failure. The optimized geometry was subjected to compressive loading condition. The gauge region showed very little shear effect in the middle and high stress concentrations at the notched ends as shown in Fig To reduce the notch effect, the gauge region was subjected to compressive force in clamped condition as shown in Fig The results improved a bit but the notch effect wasn t totally eliminated as shown in Fig Thus a double notch shear test is not the most reliable experiment for finding yield shear stress in the composite. Fig..6.5 Interlaminar and normal stress in unclamped double notch coupon [46] Fig..6.6 Clamped double notched coupon under compressive load [46]. Fig..6.7 Interlaminar and normal stress in clamped double notch coupon [46] 48
63 .7 Results The 3D linear elastic model proposed in section.4 demanded a computational time of 40 minutes on a system running with a 3.14 GHz processor. This turned out to be a major drawback of the 3D model. For the current work, the strength optimization study was carried out by Stone [46] using a D FE model based on Classical Lamination Plate Theory. Because of a large number of runs required, 3D FE model for such a study was impractical. In order to use the results of D model in the current work it was necessary to compare its results with the proposed 3D model. The basis of such a comparison was that the inplane stresses were dominant in the optimized laminate configurations until the yield point. The relevance of 3D model to strength prediction of laminates became evident when delamination was considered. P y y1 Y x x1 x longitudinal strain(ε y ), (in/in) εy D εy 3D Distance from hole along x, (in) longitudinal strain(ε y ),(in/in) εy D εy 3D Distance from hole along y, (in) (a) (b) Fig..7.1 (a) Variation of longitudinal direction strain (ε y ) along X direction using D and 3D FE model for Aluminum properties (b) Variation of longitudinal direction strain (ε y ) along Y direction using D and 3D FE model for Aluminum properties 49
64 longitudional strain, in/in εy D εy 3D longitudional strain, in/in εy D εy 3D Distance from hole along x,in Distance from the hole along y,in (a) (b) Fig..7. (a) Variation of longitudinal direction strain (ε y ) along X direction using D and 3D FE model for T600:1533 properties (b) Variation of longitudinal direction strain (ε y ) along Y direction using D and 3D FE model for T600:1533 properties Fig..7.1 draws a comparison between the D and the 3D model for longitudinal direction strain along x (from x1 to x in Fig..7.1) and y (from y1 to y in Fig..7.1). Both models used isotropic properties of Aluminum (Table.5.1). Identical results were obtained using both models. A similar comparison was drawn in Fig..7., but using T600:1533 carbon/epoxy material properties for the Baseline laminate. The 3D model prediction was 13% higher than that of the D model at point x1 and 137% higher at point y1. Point x1 is the point of the maximum strain concentration and point y1 corresponds to that of minimum strain concentration. Both the strain concentration (K t ) and the First Ply Failure (FPF) predictions were based on the point x1 and hence the 137% difference in prediction of two models was of no consequence for the current work. The difference in the D and 3D models is a direct consequence of the free edge effect which seems to be more prominent at point y1 than at x1. For the strength optimization study two approaches were used. One of the approaches had strain concentration as the governing parameter and the other was based on First Ply Failure (FPF) methodology. In the former, ply angles were altered one angle at a time and the corresponding 50
65 strain concentration factors were observed. The assumption of such an approach was that the decrease in strain concentration would mean a corresponding increase in the openhole tension (OHT) strength of the laminated composite. The laminate configurations that were obtained are given in Table.7.1 along with their strain concentration factors and the ultimate tensile strengths (UTS). Table.7.1 K t optimized layups Description Orientation K t 3D FEA UTS 5 (Ksi) Baseline (BL) [(45/90/45/0)]s Vary 45 (A) [(54/90/54/0)]s Vary 90 (B) [(45/51/45/0)]s Vary order 1 (C) [(45/0/45/90)]s Vary 0 (D) [(45/90/45/57)]s. 9 Vary 45 & 90 (E) [(54/54/54/0)]s Vary 0 & 90 [(45/5/45/5)]s Vary 0 & 45 [(6/90/6/6)]s Taking the baseline configuration and altering the 45 degree plies resulted in optimized configuration vary 45. Similarly, the nomenclature was given to the layups depending on which ply or plies were altered. An exception is vary order 1 which was obtained by changing the stacking sequence of the 90 and the 0 degree plies. Some of the laminates in Table.7.1 have also been designated as BL, A, B, C, D and E. Vary0&90 and Vary 0&45 laminates were not among the other laminates (BLE) that were fabricated. That reason being that after analyzing the vary 0 laminate it was clear that altering the main load bearing plies 6 caused drastic decrease in the OHT of the coupons. 5 The UTS is average of 3 sets of coupons that were fabricated during the course of the research. The fabrication process was completed by collaborating with Stone, D.P. [46]. 6 The load bearing plies are the one which have the fiber axis parallel to the loading direction. 51
66 Normalised to baseline Kt 0.4 UTS 0. 0 Baseline A B C D E LayUp Fig..7.3 Comparison of strength response of laminates using Kt and UTS. To compare the strength response of laminates their Kt and UTS were normalized with respect to the baseline laminate (Fig..7.3). ). Laminates A (vary 45) and B (vary 90) had a 3% increase in the strength than the baseline. Laminate C (vary order 1) which showed a higher strain concentration than the baseline had a correspondingly lower UTS (3%). Both laminates D and E were expectedd to show higher strength than the baseline due to their reduced strain concentration factors. However, in both cases the results were lower,.8% and 59 % for E and D respectively. These results indicated that the strain concentration factor method is not a reliable measure of strength for composites. To improve the optimization, failure criteria were considered. This demanded that a suitable failure criterion be chosen that could predict the strength of the laminates accurately. The D and 3D models weree linear elastic in nature. Thus, First Ply Failure (FPF) Strength was considered since it occurs in the linear range of the composites. 5
67 Fig..7.4 Load strain curve for uniaxially loaded laminate showing multiple ply failures leading up to ultimate laminate failure [34] Fig..7.5 Comparison of predicted and measured stressstrain response of [ 0 / ± 45 / 90] s glass/epoxy laminate [34] The FPF of a laminate occurs when the first ply (or group of plies) fails. Thus the load corresponding to the FPF is not necessarily the laminate failure load. Fig..7.4 shows a piecewise linear laminate loaddeformation curve with several knee points due to ply failure. The first knee point is considered to represent the FPF. Fig..7.5 shows a comparison between the FPF predicted by the maximum strain theory and the corresponding experimental data for a [ 0 / ± 45 / 90] s glass/epoxy laminate. This curve has two knee points the first one is at the strain corresponding to the failure of the 90 degree plies and the second one at the strain corresponding to the ± 45 degree plies. However unlike Fig..7.4 these knee points are not clearly defined. At high strains the experimental data does not show as much change in slope at the knees as the theoretical curve does. The actual ply failure occurs gradually over a finite strain range, whereas instantaneous ply failure at a single strain level is assumed in the analysis. To find the FPF experimentally a new technique called the digital image correlation method (DICM) was used. This technique measures specimen displacements by finding correspondence between an image of the specimen in an undeformed or reference configuration and a second 53
68 image under load. The software for the current research was provided by Correlated Solutions, Inc. The system uses two high resolution digital cameras as shown in Fig..7.6 to record surface changes of the object under investigation. The cameras were placed at an angle to focus on the hole where damage was expected to occur. 50 mm Schneider lenses Speckled composite plate Fig..7.6 Set up of the DICM instrument. DICM is based on the principle of matching the pixel grey level values of a reference image and the deformed image. To generate these pixels the surface of the specimen was coated with a layer of paint to form speckle pattern as shown in Fig..7.7 (a). The speckle should be uniform throughout the specimen and should not degrade with the application of load. 54
69 P P (a) (b) Fig..7.7 (a) Speckle pattern near the hole of Baseline laminate (b) Longitudinal strain profile of 3D model near the hole of baseline laminate at 70.5 Ksi (90 % UTS) Once the load is applied, the speckled images are registered by the software and discretized into subset. Each subset is an n n pixel window that surrounds a data point forming a strain section. Each subset of a reference image is then matched with the corresponding subset of a deformed image creating a displacement field. The displacement field information is then used to calculate strain at each data point (Fig..7.8). There are algorithms and error functions that used to perform this correlation which are explained elsewhere [46, 47, 48, 49]. Fig..6.7 (b) shows the longitudinal direction strain field near the hole of the baseline laminate at 18% UTS. Subset Fig..7.8 Steps in extraction of strain field in DICM. The subsets are spaced by a step size. Each step size denotes the increment that should be applied to a subset. This is equivalent to the elements of FEA mesh with the exception that subsets can 55
70 overlap if the step size is smaller than the subset size. A higher element density in the region of interest improves the accuracy of the solution. Similarly, a smaller step size yields more data points and better surface contours but requires more analysis time. For the current research a step size of 10 and subset size of 40 was chosen. The detailed description of the choice this subset and step size can be found somewhere else [46]. This combination resulted in higher accuracy with less computation time. From Fig..7.7 (b), the strain contours do not start from the edge of the hole. DICM can only go half a subset size from the edge of the hole, which is 0.0 inches for the subset of 40. a) b) Y X c) d) Fig..7.9 (a) DICM speckle pattern of baseline laminate with circular offset zone. (b) Longitudinal strain contour of baseline at 13 Ksi (18% UTS) (c) 3D model mesh of baseline laminate (d) Longitudinal strain contour of 3D FE model of baseline at 13 Ksi (18% UTS). 56
71 Fig..7.9 (b) and (d) compare the longitudinal strain contours of baseline laminate using DICM and 3D FEA respectively. The load in both cases was 18% of the UTS. The maximum strain concentration is 90 degrees to the loading direction (Y). To compare the FEA result the same offset was applied by calculating the node number which corresponded to the 0.0 inch distance from the edge of the hole. The best approximation of the required distance was achieved at the 5 th node from the edge of the hole. DICM and 3D FEA predicted a longitudinal strain value of and respectively at the point of interest with a difference of 3.38%. a) b) c) d) ± 45 at 7.5Ksi (41% UTS) using DICM s &3D FEA respectively (c), (d) Longitudinal strain contour for A laminate at 9Ksi (13% UTS) using DICM &3D FEA respectively Fig (a), (b) Longitudinal strain contour for ( ) 4 57
72 Fig (a) and (b) compare the longitudinal direction strain contour of DICM and 3D FEA ± 45 respectively at 41% UTS for a ( ) 4 laminate. This laminate was introduced to compare the s strain prediction of DICM and FEA and was not part of the optimization process. DICM and FEA predicted a strain of and respectively at the offset distance of 0.0 inch from the point of the maximum strain concentration. A Similar process was repeated by using laminate A at 14% UTS as shown in Fig (c) and (d). In Fig..7.9 and Fig DICM and FEA agreed well with each other in the zone of maximum strain concentration. P y1 y1 Y x x1 x longitudional strain (ε y ), in/in FEA 9% UTS DICM 9% UTS FEA 4% UTS DICM 4% UTS FEA 84% UTS DICM 84% UTS Distance from hole along X, in (a) Transverse strain (ε x ), in/in FEA 9% UTS DICM 9% UTS FEA 4% UTS DICM 4% UTS FEA 84% UTS DICM 84% UTS Distance from hole along X, in Inplane shear strain (ε xy ), in/in FEA 9% UTS DICM 9% UTS FEA 4% UTS DICM 4% UTS FEA 84% UTS DICM 84% UTS Distance from hole along X, in Fig (a), (b), (c) Comparison of 3D FEA with DICM for longitudinal, transverse and inplane shear strain respectively along X direction of the hole for BL
73 The coupons were fabricated in three groups with 4 to 5 coupons in each group. BL14 stands for the forth coupon of group one of baseline series. Fig (a), (b), (c) provide a comparison between DICM and FEA strain predictions in longitudinal, transverse and inplane shear direction respectively along X. The strains for FEA and DICM were extracted along the edge of the hole on the surface from x1 (0.15, 0) to x (0.5, 0) as shown in Fig (a). The comparison of the strain state along X was drawn for 3 load steps of 7ksi (9% UTS), 17 Ksi (4% UTS) and 60 Ksi (84% UTS). The longitudinal strain was positive for all load steps as expected for a tensile loading condition while the transverse strain was negative due to the Poisson s effect. In Fig (a) the correlation between 3D FEA and DICM changed from 1% at 7ksi (9%UTS) to 38% at 60Ksi (84% UTS). For the transverse strain the difference ranged from 10% at 7Ksi (9% UTS) to 56% at 60 Ksi (84% UTS). For the inplane shear the difference corresponding to 84% UTS was 10% making it the worst case scenario Longitudinaldirectiona strain(ε y ),(in/in) DICM 3D FEA 90 % UTS Distance from hole along x,(in) Fig..7.1 DICM Vs 3D FEA for laminate A 59 50% UTS 5% UTS 10% UTS
74 Fig..7.1 compares the longitudinal direction strain between DICM and 3D FEA model for 10%, 5%, 50% and 90% of the UTS. Laminate A was selected for this comparison. The longitudinal direction strain profile between DICM and 3D FEA agreed well till 5% UTS. At loads approaching 90% UTS the correlation deteriorated. From Fig (a), (b), (c) and Fig..7.1 it is clear that the DICM and 3D FEA correlate well with each other under 5% UTS. At higher loads ( 84) geometric and material nonlinearity effects lead to poor correlation between the two methods. Using DICM, FPF was defined as the point where the proportional line and the stressstrain curve deviated from each other. Fig shows the applied stress Vs longitudinal strain curve for the three sets of baseline laminates that were fabricated for this work. In depth study of the use of DICM for obtaining the stressstrain curves and deriving FPF from them can be found in [46] σ y (psi) Proportional line FPF line ε y (in/in) Fig Applied stress Vs Longitudinal strain for set of Baseline laminates [46] The purpose behind using the DICM for OHT test was its ability to spatially extract strains near the edge of the hole where the damage was expected to occur. These predictions could then be 60
75 compared with the FPF prediction of the failure criteria introduced in sections and The failure criteria application for the current work was concentrated near point A (Fig..3.5). The 3D model had two elements per ply as shown in Fig which meant that each ply along the edge of the hole had 3 nodes of which were shared with the neighboring plies except for the free edge plies. P. Plane of Symmetry Fig FE mesh of oneeighth model near the edge of the hole for baseline laminate. A static load applied to the FE model in the y direction produced a 3D strain state at each node along the edge. The strains extracted from ANSYS were in the reference coordinate system (X YZ). The values were converted into the principal material coordinate system by using 3D form of equation.3.4. For a node shared by two plies this transformation resulted into two strains one for each of the plies that share it. It is because the transformation matrix T 3D 61 is a function of ply angle and would thus generate two sets of strains for the shared node. Principal stresses were obtained from principal strains from equation.3.3. Each failure criterion generated a failure index (f.i) at each node along the edge of the hole. The tendency of failure was governed by the
76 magnitude of f.i. The node with highest f.i would have the tendency to fail first and hence result in FPF. The FPF stress was calculated for each node by the equation. P FPF = (.7.1) f. i. where P is the applied tensile stress as shown in Fig and f.i is the failure index which is defined as ε. ifea σ f i= = ifea (.7.) ε imax. σ imax. ε ijfea σ ijfea f. i= = (.7.3) ε σ ijyield. ijyield where i, j = 1,, 3. Equations.7. and.7.3 were used for maximum strain and maximum stress failure theories. As explained in section.3 the normal stress and strain components show linear behavior and hence their ultimate or maximum stress and strain values can be used to find the failure index as shown in equation.7.. However, we have found that the shear is nonlinear in nature and hence to find the f.i. in this case the stress and strain values should be divided with the corresponding yield stress and yield strain as shown in equation.7.3. Failure index for the interactive criteria is the left hand side of their 3D failure criteria equations. Table.7. provides comparison between the FPF strength of layups optimized by strain concentration method. Fig provides the same comparison in graphical form. The error bars in Fig are the standard deviations of 3 sets of coupons tested using DICM. The FPF predicted by the DICM [46] agreed well with that predicted by MaxStress and MaxStrain theories. HashinRotem, TsaiHill, TsaiWu and Hoffman under predicted the FPF strength of all the laminates. The energy criterion results were also conservative for all but one laminate (Laminate C), for which case the FPF strength was over predicted. 6
77 Table.7. FPF strength values for Kt optimized laminates using DICM and 3D failure criteria. layup DICM MaxStress Max MaxStrain HashinRotem TsaiHill TsaiWu Hoffman Energy Baseline A B C D E First Ply Failure Strength, (ksi) 5 DICM MaxStress Stress 0 MaxStrain Strain 15 HashinRotem Rotem TsaiHill 10 TsaiWu 5 Hoffman 0 Energy Baseline B Layup C A D E Fig Comparison of FPF strength of Kt optimized laminated using DICM and failure theories. Of the two theories, MaxStrain Strain was able to predict FPF more accurately than MaxStress. Max Thus the optimization study was continued using the Max MaxStrain Strain theory with FPF strength as the FPF Strength, (Ksi) governing parameter DICM MaxStrain F G Layup H Fig Comparison of FPF of laminates optimized using Max MaxStrain Strain theory with DICM. 63
78 Fig compares the FPF strength of the laminates optimized by the MaxStrain criterion. Laminate C (vary order 1) was found to have higher FPF strength than the baseline. This supported the theory than stacking sequence change can alter the FPF. Vary order (Laminate F) was thus included in the current study to observe the effects of further change in the stacking sequence. It was not the part of K t or FPF optimization methodology. Using the MaxStrain theory the orientation of 45 and 90 degree plies was altered to find maximum FPF. Laminate G was obtained by varying the 45 and laminate H was obtained by varying the 90 degree ply. Varying 0 degree layer reduced the FPF and UTS and thus was not considered. H had the greatest improvement in strength, 97% higher than the baseline FPF. It was followed by laminates E, B, G, and C with 69%, 5%, 31% and 8% increase in FPF strength respectively than the Baseline. Laminates A, D and F had FPF strength lower than the baseline by 9%, 38% and 4% respectively. The final set of laminates is summarized as Table.7.3 Final set of fabricated laminates along with the method of optimization. Orientation layup Optimization method [(45/90/45/0)] S Baseline  [(54/90/54/0)] S A Kt [(45/51/45/0)] S B Kt [(45/0/45/90)] S C literature [(45/90/45/57)] S D Kt [(54/54/54/0)] S E Kt [(45/45/90/0)] S F literature [(1/90/1/0)] S G FPF [(45/0/45/0)] S H FPF 64
79 Table.7.4 Mode of first ply failure along with the ply failed. Orientation Layup FPF Stress (Ksi) Ply Failed at FPF Mode of FPF [(45/90/45/0)] S BL ε [(54/90/54/0)] S A ε [(45/51/45/0)] S B ε 1 [(45/0/45/90)] S C ε [(45/90/45/57)] S D ε [(54/54/54/0)] S E ε 1 [(45/45/90/0)] S F ε [(1/90/1/0)] S G ε [(45/0/45/0)] S H 345 ε 1 Maxstrain failure theory was also used to find out the modes of first ply failure and the laminae which were supposed to fail at FPF load (Table.7.4). According to MaxStrain failure theory FPF in most of the laminates was predicted to occur transverse to the fiber direction, indicating matrix cracking. However, as shown in Table.7.4 some laminates had tendency to have FPF in form of inplane shear. From the optimization study and the mode of FPF failure of the laminates some conclusion could be drawn. In case of H laminate the 90 degree plies were replaced with the 0 degree plies that dramatically enhanced it load bearing capability. Apart from H the other laminates that showed increase in FPF strength were E, B, G and C. Again G was optimized by MaxStrain theory and thus its FPF strength increase was not surprising. However, the FPF results of laminates E, B and C that were optimized using K t were quite surprising. In laminates B and E the FPF failure mode was inplane share, the same as in case of laminate H. This can be due to shifting of 90 degree plies. In all other laminates with 90 degree plies, the FPF failure mode was transverse in nature which would mean matrix cracking and relatively lower resistance to applied stress than an inplane shear mode where the fibers would redistribute some of the applied stress in the lamina and increase its resistance to failure. In laminate C it seems that moving the 90 degree laminate further inside and away from the free edge lead to higher FPF. Apart from these there were laminates that performed poorly in terms of FPF strength. As 65
80 mentioned earlier laminates A, D and F had FPF strength lower than the baseline. D laminate had the lowest K t and still was the weakest of all the laminates. Due to removal of the primary load bearing plies this laminate basically behaved as a shear coupon and showed least FPF and UTS strength. In laminate A ± 45degree laminae were replaced by ± 54 degree plies. This seems to have lowered the FPF strength as the plies were moved away from the main load bearing angle Failure Index (f.i) BL A C D F G Distance from the hole along X, (in) Fig Failure Indices (f.i) Vs X distance along the hole at the lamina location where FPF is predicted in transverse mode Failure Index (f.i) Distance from the hole along X, (in) B E H Fig Failure indices (f.i) Vs X distance along the hole at the lamina location where FPF is predicted in inplane shear mode 66
81 Fig shows the variation in the failure indices (f.i) along the x axis at the location along the edge of the hole where MaxStrain theory predicted FPF in transverse direction. Fig provides the similar comparison for laminates where FPF was expected in shear. Both these figures provide a qualitative method of comparing laminates having higher FPF when all layups were exposed to the same load. In Fig the D laminate showed the highest failure index in the transverse direction in a 90 degree ply. Laminate G showed a minimum failure index in the 90 degree ply which obviously contributed to its high FPF. In Fig the f.i of the 54 degree ply of B laminate was higher than that of 45 degree ply of E laminate which in turn was higher than the f.i. in 45 degree ply of H laminate. The FPF strength followed the reverse order with H being the strongest and B being the weakest. The plots in Appendix A3 compare the failure indices (f.i) of the laminates involved in this study. These failure indices were determined at the location near the edge of the hole where MaxStrain failure theory predicted FPF. The failure indices have been derived for all six strains (3 normal and 3 shear) along X direction (Fig (a)) of the hole. By comparing the f.i. derived for strains in 1,, 3, 1, 3 and 13 directions one can observe that among all the laminates involved in this study, failure modes in transverse () and inplane shear (1) direction dominated the FPF. An important observation was with regard to laminate G where the f.i in out of plane shear (3) direction was very close to the f.i of transverse () direction. This meant that the interlaminar shear in this laminate could affect its strength as the damage progressed. G laminate has been treated separately in section 4.4. The FPF mode was verified using SEM. The region of interest was the edge of the hole at 90 degrees to the loading direction (y direction). The process of creating specimen for SEM analysis is explained in section 3. of chapter 3. Before sectioning, the laminates were subjected to the FPF load. If the predicted FPF was correct, cracks would be visible at the desired location. 67
82 Y Y X Fig Crack in the 90 degree ply of baseline laminate in direction at FPF Fig..7.0 Crack in the 45 degree ply of H laminate in 1 direction at FPF Fig shows a crack in the 90 degree lamina in baseline laminate in transverse () direction. The load was acting in the Y direction as shown in the same figure. The FE model predicted the FPF at the node shared between 45 and 90 degree lamina. From the image it can be assumed that the crack initiated at the interface of 45/90 lamina and propagate through the 90 degree lamina splitting it along transverse direction. Fig..7.0 shows a crack at the interface of 45 and 0 degree lamina of the H laminate. The 3D FE model for H laminate using MaxStain theory predicted FPF at the interface of 45 and 0 degree lamina in form of inplane (1) shear. 68
83 Strength, Ksi UTS Reference line FPF Maxstrain UTS FPF Reference line 0.00 Baseline A B C D E F G H LayUp Fig..7.1 Trend followed by FPF and UTS of laminates Fig..7.1 compares the FPF predicted by Max MaxStrain train theory of the 3D FE model with the measured UTS. The FPF and the UTS reference lines are to compare with the baseline layup. la Lay ups A, D and F have FPF strength less than the Baseline. The UTS of layups lay A and F is higher than the baseline while that of D is lower than the baseline. B, C, E, G and H have FPF strength higher than the baseline. The UTS of B, G and H is high higher er than the baseline UTS while that of C and E is lower. This indicated that although increasing FPF is a novel method of finding laminates that can resist damage initiation but it is not a guarantee that the laminates having higher FPF will have a higher UTS too. For most applications the FPF methodology of strength optimization is a conservative one. 69
84 .8 Chapter Summary A 3D linear elastic model was proposed to capture the through thickness strain field near the hole of the composite plate. The model was linear elastic in nature and compared well with the analytical solution as well as with the experimental method (DICM). 3D model and DICM had good correlation for applied stresses less than 5% UTS. At stresses approaching 50% and higher this correlation degraded due to material and geometric nonlinearity. The model evaluated the strength response of nontraditional laminates using strain concentration factor and FPF strength methodology. Strain concentration factor was not found to be a reliable test of the strength of a laminate e.g. the D laminate had the lowest strain concentration factor and was still the weakest of all the laminates. Hence, an FPF based study should be preferred. Seven failure criteria were used to estimate the FPF strength of the laminates. MaxStrain failure theory was found to correlate best with the FPF predicted by the DICM. MaxStrain failure theory was also able to predict the location and the mode of FPF near the hole of the composite laminate. SEM was used to verify the mode of failure results for baseline and H laminate. Both laminates had FPF at the locations and in the mode in which they were predicted by the 3D model. The chapter ended with a note of caution that the FPF and the UTS of a composite laminate may or may not be linearly related. Increase in FPF strength can lead to increase in UTS like in laminates B, G and H whereas in some laminates like C and E, the UTS was found to be lower than the baseline even though they had a comparatively higher FPF. 70
85 3. Manufacturing 3.1 Fabrication Fig Schematic of fabrication set up [50] The composite plates were fabricated using hand layup system. Fig shows the schematic of a typical hand layup system. This system involved lying plies of precut prepreg into a mold. Prepreg stands for preimpregnated materials. They are reinforcement fibers or fabrics into which a precatalyzed resin system has been impregnated by a machine. The prepreg resins can only be fully cured by heating them to the prescribed cure temperature. Prepreg is usually rolled into tape and kept in a freezer to slow down the cure process. Care should be taken while handling the prepreg material as direct contact with hand can contaminate them and degrade the material properties. Prepreg was cut to form plies of desired angles on a clean table to prevent contact with any impurities. The mold or tool was an aluminum plate of 30.5in 8in 0.5in dimensions. Before placing the plies on the mold it was cleaned with acetone. A water based P.T.F.E. mold release agent was applied on the mold. Care was taken than no air bubbles formed on the surface as this could lead to nonuniform application of release agent. Mold release agents 71
86 are thermally stable and can withstand a temperature of F. Mold release was allowed to dry up for 0 minutes. The plies were stacked on top of each other to form the part as shown in Fig Pressure was applied on the stack of plies with a roller to take out any voids between two prepreg layers. Voids cause nonuniform properties and also reduce the fiber volume fraction. Release film or peel ply covered the laminate stack. The purpose of peel ply is to provide a simple method of removing the bagging material off the part after curing. Generally, the release film material is porous to permit excess resin to flow through it. As shown in Fig a breather cloth covered the peel ply and a vacuum valve was placed on top of it. The breather material acted as distributor for air (vacuum) and for escaping volatile gases. Butyl tape was placed around the part. It acted as a sealant. The whole part was then covered by vacuum bagging. A small cross shaped cut was made on the vacuum bagging so that a vacuum valve would fit into vacuum nozzle. After the bagging system was assembled it was placed in the autoclave for curing. The curing process used both vacuum and heat. Vacuum helps in consolidating the laminate s layers. This reduces the void content in the composite. This is important as interlaminar shear strength reduces by 7% for each 1% of void content present up to maximum of about 4%. A reasonable goal for void content in the finished laminate is 0.5% or less [50]. The curing was carried out at F and 90 Psig. The process started with a 10 minute ramp period with a soaking time of 45 minutes. This was followed by a slow cooling for another 45 minutes. After the part was cured the laminate plate was taken out and sent to WSU machine shop for cutting in 1in 1.5in plates. Waterjet system and an aerospace quality abrasive mixture was used for the cutting operation. The holes were drilled using a drill press. 7
87 3. SEM Sample Preparation Y X A B A B 1 3 Fig Steps in preparing SEM sample for FPF and Delamination study Fig.3..1 shows the stages in preparing samples for analysis using SEM. The load was applied along Y direction. The laminates were first subjected to FPF or Delamination initiation load and then taken to a diamond saw cutter where two pieces were cut near the hole marked as A and B in image 1 of Fig Care was taken while cutting near the hole so that the cutting process itself won t introduce any damage. The edge of the hole was not exposed to the cutter so the point was slightly depressed relative to the sample surface. Two white dots were put on the depressions as shown in image of Fig An epoxy mold was prepared by mixing 6ml hardener with 35 ml resin. The two samples from image were placed in 3M TM ScotchWeld TM translucent epoxy adhesive with the dots facing down. Once the epoxy cured, the samples were ground to expose the dotted layer. Samples were polished with a 1µm solution, followed by a 0.05µm solution and finally a 0.03µm solution. The samples were cleaned in an ultrasonic cleaner and then rinsed with alcohol. Pressurized air was used to dry the samples. Before mounting the samples in the SEM, a conductive link was placed between the samples and the 73
88 base of the sample. This was done by running a strip of carbon tape all the way round the epoxy so that it touched the samples and the holder on which it was to be mounted. Image 3 in Fig was a sample for G laminate. The surface of the sample was sputtered with gold. Sputtering is a technique of applying a molecular layer of atoms to a surface. The image of the crack before sputtering was very blurry. Sputtering improved the electrical conductive of the sample and resulted in a much better image. Due to cost concerns this technique was used only for G laminate. The SEM images of other laminates used in this study (Baseline, H) were clearly visible without any sputtering treatment. Use of sputtering for other laminates (A, B, C, D, E, F) was redundant as damage due to manufacturing defects or during sample preparation made them unfit for further analysis. 74
89 4. Delamination 4.1 Introduction A limitation of D models is that stresses in the zdirection are neglected (Fig.4.1.1). The accuracy of the D model decreases in regions with geometric discontinuitiess and free edges. Free edge perturbations decay rapidly with the distance from the laminate edge. These out of plane stresses are responsible for premature failure of laminates in the form Pipes and Pagano [51] used a 3D elasticity approach to quantify interlaminar of delamination. stress fields near free edges. Fig Pipes and Pagano model for analysis of interlaminar stresses in a laminate under uniaxial tension [51] 75
90 The three stress equilibrium equations from the theory of elasticity are [51] σ X τ XY τ XZ + + = 0 X Y Z (4.1.1) τyx σy τ YZ + + = 0 X Z Z (4.1.) τ ZX τyz σ Z + + = 0 X Y Z (4.1.3) The laminate in the Pipes and Pagano model was loaded uniaxially in the x direction and stresses σ X near the free edge y = ± b were considered. Since load does not vary along x, = 0. Thus X from equation 4.1.1, interlaminar shear stress τ ( z ) is given by XZ ( z Z τ XY τ XZ ) = Y dz (4.1.4) t The inplane shear τ XY has a constant value given by Classical Lamination Plate Theory in the interior regions of the laminate. As y approaches ± b, τ XY must decrease to zero. In other words as y ± b, τ Y XY must increase. From equation we can conclude that τ XZ must increase from zero in the interior of the laminate to large value as y ± b. From equations 4.1. and 4.1.3, the other interlaminar stresses are ( z Z σ Y τyz ) = Y dz (4.1.5) t ( z Z τ YZ σ Z ) = Y dz (4.1.6) t 76
91 Pipes and Pagano [51] used a finite difference numerical scheme to solve the three governing equations. The distribution of inplane and interlaminar stress in a ± 45 degree laminate by Pipes and Pagano s elasticity solution is shown in Fig As explained earlier τ xy is expected to decay to zero near the free edge of the laminate while τxz is expected to progressively increase near the same edge. Both these stresses were calculated along the interfaces of +45/45 degree lamina. Fig.4.1. Distribution of stress in free edge region by elasticity method [51] 4.. Finite Element Comparison Analytical results obtained by Pipes and Pagano [51] were compared with the 3D FEA solution. The model introduced in chapter was for a composite plate with a hole in it. However, the analytical results derived by Pipes and Pagano were for an unnotched composite plate. Hence, the hole in the geometry of the 3D model was eliminated to obtain an unnotched geometry for FE analysis. In order to maintain consistency in the coordinate system used in chapter, the coordinate system of the unnotched laminated plate was not altered. It should thus be kept in mind that the X axis of the analytical solution used by Pipes and Pagano corresponds to Y axis of the 3D model. The interlaminar stresses were determined by FEA for the [ ] / 45 / 45 / 45 s
92 laminate using the properties of T600/1533 material given in Table.3.1. Fig.4..1 shows the geometry used for comparing the FEA results with the analytical results in Fig.4.1. [51]. The dimensions of the FE model of chapter were retained for this analysis. Fig.4..1 also shows the BCs used for the unnotched FE model. Symmetry was used along the three mutually perpendicular faces of the model. Since the comparison was for the [ ] 45 / 45 / 45 / 45 s layup, only 4 layers were included in the FE. The width (b) of the model was 0.75 in, height was limited to 1.5 in and the thickness (h) of the 4 laminae was in. Solid 64 brick element was used. The model was subjected to a tensile stress (P) of 30,000 psi along ydirection. P P s s s s s s in s s s s s s y s s x s s A s y z B b=0. 75 in h= in Fig.4..1 Geometry and BCs used for FEA of unnotched [ ] 45 / 45 / 45 / 45 s laminate. The inplane stress τ XY and interlaminar shear stress τ XZ were plotted with respect to distance from free edge as shown in Fig.4... The coordinate system followed for the plots in Fig
93 is shown in Fig Free edge is denoted by point A in Fig and B denotes a point at the plane of symmetry. Both A and B lie at the interface of +45 degree and 45 degree lamina. The region near the free edge where the change in stress field was appreciably higher is the boundary layer. This region was approximately twice the thickness of laminate. The results from Fig. 4.. were compared with the stress distribution in Fig FEM results confirmed the predictions of Pipes and Pigano that as one moves closer to the free edges of a laminated composite, the inplane shear decreases rapidly and the interlaminar shear stress simultaneously increases. In Fig.4.. y/b = 0 represents the free edge and y/b=1 represents the plane of symmetry shear stress,psi shear xy shear yz Plane of symmetry (Point B in Fig. 4..1) Free Edge (Point A in Fig. 4..1) Boundary Layer y/b, in/in Fig.4.. Distribution of stresses in the free edge region by FEM for [+45 0 /45 0 /+45 0 /45 0 ] s Pipes and Pagano [5] also considered the [+15 0 /15 0 /+45 0 /45 0 ]s laminate They kept the loading condition the same as that for [+45 0 /45 0 /+45 0 /45 0 ] s which is shown in Fig They used the elastic coefficients of Foye and Baker [53], namely, 79
94 E L = Psi, E T = Psi, G LT υ LT = 6 = Psi, 0.19 where L is fiber direction, T is transverse direction and υ LT is the major Poisson s ratio. Placing ± 15 0 on the outside they observed that for b/h > 10 the interlaminar stress ( σ Z ) resembled the plot shown in Fig For small ratios the authors [] predicted a steep gradient near the free edge with infinite stress value at y / b=± 1. Fig.4..3 Predicted variation of interlaminar normal stress field along y [5] The stress field was compared with the FEM solution which was obtained by replacing the [+45 0 /45 0 /+45 0 /45 0 ]s orientation by [+15 0 /15 0 /+45 0 /45 0 ]s. Interlaminar normal stress between /15 0 interface was plotted as a function of x/b (y axis of Pipes and Pagano corresponds to x of FE solution) for two b/h ratios. In Fig.4..4, x/b = 0 symbolizes the free edge and x/b=1 is the plane of symmetry σ z, (Psi) b/h= b/h= x/b, (in/in) Fig.4..4 Variation of interlaminar normal stress along x for different b/h ratios 80
95 4.3 Notch Effect: As shown in the preceding sections, analytical work has been done in the area of the free edge effect and delamination occurring in unnotched laminates. The FE model results agreed well with the analytical model predictions. However the main focus of this thesis was to estimate the effect of notches on interlaminar stresses and ultimately delamination. It has been found that the presence of discontinuities such as holes, ply drops and joints results in higher interlaminar stresses and thus increases the probability of delamination [54] εz notched baseline εz unnotched baseline Notch εxz notched baseline εxz unnotched baseline Interlaminar strain, (in/in) Distance along x, (in) Fig Interlaminar strain comparison between notched and unnotched coupon. Fig provides a comparison of the interlaminar strain between the notched and unnotched baseline laminate. The interface between (0 0 /45 0 ) lamina was considered in this case. Both plates were of the same half width b. The presence of high outofplane shear and normal stresses near the hole clearly indicates the sensitivity of interlaminar stress to the presence of any notch in the body. 81
96 4.4 Results Delamination is an initiation and growth process. After initiation, the delamination can undergo stable growth. Eventually due to unstable growth and interaction with inplane failure modes, the final fracture occurs [55]. There are two basic approaches to predict delamination in laminates. Some use a mechanics of materials approach. Using strength parameters the local state of stress in the nterplay matrix layer where delamination occurs is found [56]. Others have used fracture mechanics techniques. The most common approach involves the strain energy release rate. O Brian [57] derived a single equation for the calculation of the total strain energy released per unit delaminated area along a straight edge: t ε G= ( ELAM EW ) (4.4.1) where G is the strain energy release rate or energy per unit delaminated area, t is the laminate thickness, ε is the longitudinal strain level, E LAM is the longitudinal modulus of the undelaminated laminate and remaining after delamination. E W is the weighted average longitudinal modulus of the sub laminate O Brian has shown that critical values of the strain energy release rate are in fact laminate dependent and has suggested that critical strain energy release rate (G c ) is a function of the percentage of the total strain energy release rate that can be attributed to mode І. However for the current work a mechanics of materials approach. The reason being that in composites a large number of failure modes coexist and thus a fracture based approach would not be able to provide an accurate solution. Quadratic Delamination Criterion is based on mechanics of materials. 8
97 4.4.1 Quadratic Delamination Criterion Brewer and Lagace [55] proposed the Quadratic delamination criterion which can be written as σ σ σ T 3C or σ + + = 1 S S S S T 3C (4.4.) where σ 13 and σ 3 are interlaminar shear stresses, σ3t and σ 3C are interlaminar tensile and compressive normal stresses respectively, S 13 and S 3 are interlaminar shear strengths, are interlaminar tensile and compressive strengths respectively. Transverse isotropy was assumed, so that: S 3T T S3T and S 3C = S (4.4.3) S = S (4.4.4) 3C C where ST and S C are ultimate transverse strengths in tension and compression. The authors in [55] also observed that: S13 = S3 = S1 (4.4.5) where S 1 is the in plane shear strength as given in Table.3.1. Fig shows that interlaminar stresses near notches are higher than the interior of laminates. So, quadratic delamination criterion was applied near the edge of hole and throughout the thickness of the FE model as shown in Fig The delamination initiation stress ( σ ) is predicted by D σ D = P / f. i (4.4.6) where P is the applied tensile stress and f.i. stands for the failure index and is equal to the left hand side of the equation 4.4. for a given P. Delamination initiation was expected at the 83
98 interface separating two lamina. So the quadratic failure criterion was applied to the nodes separating two layers Fig Edge of the hole near the point of maximum strain concentration. Fig shows the elements of the 3D model stacked together through the thickness of the laminate near the edge of the hole. The numbers 1,, 3, 4 stand for the material layers of 45, 90, 45 and 0 respectively for a baseline laminate. The arrow points to the node which is shared by the 45 and 90 degree lamina and there are 7 such nodes shared by different lamina. These nodes were used to evaluate the quadratic delamination criterion using equations Layup Table Delamination initiation stress along with the interfaces delaminated. FPF using MaxStrain (Ksi) Delamination stress (Ksi) DICM UTS(Ksi) Interface delaminated BL (45/90) A N/A B N/A C (0/45) D (45/90) E N/A F N/A G (1/90) H N/A 84
99 Table provides a comparison of the delamination initiation stress of the layups with their corresponding FPF and UTS. The lamina interfaces that showed the highest failure ratio were assumed to delaminate first. 350 FPF Delamination Initiation Stress UTS Stress, Ksi BL A B C D E F G LayUps H Fig.4.4. Comparison between FPF, UTS and Delamination initiation stress of different layups Fig.4.4. shows the comparison between the delamination initiation stress of different layups with the FPF strength calculated by the maxstrain theory of 3D model and the ultimate tensile strength (UTS). The laminates designated as BL, C, D and G show delamination initiation at 71%, 96%, 57% and 17% of the UTS respectively. Laminates A, B, F and H have delamination initiation stress higher than UTS which indicates that these laminates should not delaminate at all. Laminate D and G have a delamination initiation stress very close to the first ply failure. 85
100 0.01 P Interlaminar Strain, in/in Notch end εz BL εxz BL εz G εxz G Y x A Distance along X, in Fig Comparison of interlaminar strains between Baseline and G laminate Fig compares the interlaminar strains between the [45 0 /90 0 ] interface of the baseline and the [1 0 /90 0 ] interface of the G laminate. FE models of both the laminates were subjected to a uniaxial tensile stress of Psi. As shown in Table 4.4.1, delamination was expected to initiate along these interfaces in these two laminates. The Baseline was chosen as a reference laminate and the G laminate was chosen as it showed the lowest delamination initiation stress. This made the G laminate prone to delamination. From Fig it can be observed that G laminate experienced a lower interlaminar normal compressive stress and a higher interlaminar shear stress than the Baseline laminate. Interlaminar shear is always harmful for the delamination strength of the laminated composite. On the other hand normal compressive stress increases the resistance of the laminate against delamination failure. Keeping this in mind one can explain the lower delamination strength of the G laminate than the Baseline. 86
101 The accuracy of the predictions of the quadratic failure criterion was provided by SEM images. Laminates BL, C, D and G were loaded up to the delamination initiation stress and examined using SEM. Due to some damage while preparing the sample for SEM the images of laminates C and D couldn t be examined Fig Crack between the 45/90 degree interface of baseline laminate Fig shows a hairline crack at the interface of 45 and 90 degree laminae. The right hand side of the image shows a section of the crack where it can be seen to propagate into the 45 degree lamina. However, it is quite difficult to determine if the delamination initiation at the  45/90 interface occurred first and then led to the crack propagation inside the 45 degree lamina or vice versa. The Quadratic delamination criterion for this research was based on linear elastic FE model. If delamination in a laminate occurs after the FPF, the accuracy of the predicted stress at which delamination initiationn takes place would decrease. In such situation the qualitative results should be used to compare the relative response of laminates to Delamination. The Baseline laminate is one such example where delamination is supposed to set in at 71% of UTS. 87
102 Fig Crack between the 1/90 degree interface in baseline laminate. Fig G laminate at ultimate load Fig shows a crack between the 1 and 90 degree layers of the G laminate when the laminate was subjected to a delamination initiation stress of Ksi. In the right hand side image of Fig it can be seen that the crack propagated through the 1/90 interface and then entered the 90 degree lamina. Fig shows the ultimate failure mode of G laminate. The final failure was due to delamination resulting in separation of the individual laminae. This result 88
103 confirms that the delamination initiation stress of the G laminate was very close to the FPF. The onset of delamination at such an early stage resulted into a catastrophic failure. Fig Laminate A at ultimate load Fig Laminate E at ultimate load 89
104 Fig shows the front view and the side view of the laminate A (Vary 45) when subjected to ultimate tensile stress of 73 Ksi. Fig shows the front and the side view of laminate E (vary 45 & 90) when subjected to an ultimate tensile stress of 68 Ksi. According to Fig.4.4. quadratic delamination criterion predicted the delamination strength of both laminates A and E higher than their corresponding UTS. This result was used qualitatively to suggest that these laminates won t delaminate. By comparing Fig.4.4.6, Fig and Fig it can be clearly seen that unlike G laminate, laminates A and E didn t fail in delamination. This validates the methodology of estimating the response of a notched laminate to delamination failure. 4.5 Chapter Summary The ability of a 3D model to capture free edge effects makes it an ideal tool for studying interlaminar stresses which may lead to delamination failure. For the current study, the linear elastic 3D model proposed for a composite plate with a circular notch was further used to predict delamination initiation stress. The laminates selected from the K t and FPF optimization study were used as test samples. Sensitivity of interlaminar stresses to the presence of notch was shown which lead to the belief that the edge of the hole (the one perpendicular to the loading direction) should be prone to delamination failure if any. Quadratic delamination criterion was selected that allowed to compare the relative response of laminates to delamination. One particular laminate G was expected to show a final failure in form of delamination. SEM was used to validate the claim. 90
105 5. Computational Micromechanics 5.1 Introduction Stress and deformation analysis of fiber reinforced composites is carried out at different levels. The detail necessary for the description of composite material depends on the level of post processing desired. Fiber reinforced composites can be studied as homogenous or heterogeneous bodies. When treated as homogenous, fiber and matrix are not considered separate and effective elastic properties like Young s Modulus( E ), shear modulus ( G) and Poisson s Ratio ( υ ) of the whole lamina are used for numerical analysis. To determine the effective properties (as shown in Table.3.1) of the lamina, experimental procedures similar to the one described in section.3 are used. Treating composites as heterogeneous media is a rather tedious and expensive process and in most cases homogenous models provide sufficient information to tackle design problems. However, by using heterogeneous models and the elastic properties of the constituent fibers and matrix, the homogenous properties of the lamina can be determined. This is intended to replace the experimental procedure for achieving the same results. The process of using the microstructure to determine the homogenous properties of the composite lamina is called micromechanics and the models proposed for this process are called micromechanical models. These models are classified as empirical, semiempirical, analytical and numerical. This chapter is aimed implementing micromechanics as a FE based model. The model can be used to crosscheck the elastic properties of a composite material system and also to visualize the effect of the applied strain state at the fiber and matrix level. 91
106 5. Numerical Homogenization In most commercially fabricated composites, it is not possible to control the placement of fibers very precisely. Fig.5..1 shows the random distribution of fibers in the 90 degree lamina of the baseline laminate. The fiber diameter of T300 fibers in Fig.5..1 was found to be 6.95µm. For this work the fiber diameter was rounded off to 7µm. Fig.5..1 Random distribution of fibers in 90 degree lamina in baseline laminate Some [58, 59] have documented that a random microstructure results in transverse isotropic behavior at the mesoscale and a hexagonal array of fibers has been found to simulate this behavior at the microlevel. This is important from the point of view of this study as the stiffness matrices for different laminae in equation.3.8 depicted transverse isotropic behavior. From Hook s law the transverse isotropic stiffness tensor can be obtained given by 9
107 _ _ σ 1 ε _ C 11 C 1 C 1 _ σ C 1 C C ε _ C _ 1 C 3 C σ 3 ε 3 _ = ( C C 3) σ γ 4 _ C 66 0 σ γ 5 5 _ C 66 σ γ 6 6 (5..1) The subscripts 1,, 3 are the normal and 4, 5, 6 are the shear components of stress and strain with tensor strains γ 4 ε 3, γ 5 ε 13 and γ 6 ε = = = 1. The over bar denotes that average of the terms is computed over the volume of a representative volume element (RVE). For this study the RVE is a section of the hexagonal array which represents the behavior of the whole cell. Fig. 5.. shows a hexagonal array of fibers embedded in matrix. Fig. 5.. also shows a section of the hexagonal array which formed the RVE for the current study. RVE Fig.5.. Composite material with a hexagonal array of fibers [58] 93
108 The RVE based FE model was used to determine the components of the stiffness tensor of the equation The elastic properties of the homogenized material were then determined using the following relations [58] C1 E1 = C11 C + C 3 (5..) E ( + ) ( ) C C C C C C = C11C C1 ν ν = = 1 C 1 ( C + C ) 3 ( C11C 3 C1 ) ( C11C C1 ) 3 (5..3) (5..4) (5..5) G = C (5..6) 1 66 where E1 and E are the longitudinal and transverse Young s moduli, ν1 and ν3are the longitudinal and transverse Poisson s ratios and G1 is the longitudinal shear modulus of the composite lamina. Since the body is transversely isotropic, therefore E = E (5..7) 3 ν1 = ν13 (5..8) G = G (5..9) 1 13 and G 3 E = 1 ( + ν ) 3 (5..10) 94
109 5.3 RVE Geometry a Matrix Z Y Fiber X 60 0 a 3 Fig Geometry of RVE The Fiber volume fraction ( ν f ) is defined as the ratio of the volume of fibers to the volume of composite. The dimensions a 1, a and a 3 of the RVE were chosen to obtain a particular fiber volume fraction with a hexagonal array. For the RVE in Fig with a fiber diameter d f, the volume of fibers is a 1 V f = π d a 1 4 f (5.3.1) = aπ d (5.3.) 1 f The unit cell volume, Vc is V c = 1 3 a a a (5.3.3) From which the fiber volume fraction can be found as = 8a1a a 3 (5.3.4) ν f = V V f c π d f = (5.3.5) 8a a 3 95
110 For most of the commercially available composites, a fiber volume fraction of 0.65 is used. Therefore, equation can be rewritten as π d f 8a a 3 = 0.65 (5.3.6) From Fig the relationship between a and a 3 can be established as a = a 0 3 tan 60 (5.3.7) The dimension a 1 is chosen arbitrarily. For the current study a 4 a 1= (5.3.8) Using equations 5..6, and and assuming a fiber diameter of 7µm we get a1 = 1.033µ m, a = 4.134µ m and a3 = 7.16µ m. These dimensions were used to generate the geometry of the RVE. 5.4 Material Properties The elastic properties of the constituent fiber and matrix of T600:1533 were unavailable. From the literature [34] it was clear that both T300:934 and T600:1533 had almost identical homogenized elastic properties. For the RVE model the elastic properties of the constituent fibers and matrix of T300:934 (Table 5.4.1) instead of T600:1533 composite material were used. Table Elastic properties of constituent fibers and matrix of T300:934 composite material Fiber 6 6 E f 1 = Psi E f =.0 10 Psi, E f 3 = E f 6 G f 1 = Psi, G f 13 = G f 1 6 G f 3 = Psi υ f 1 = 0.0 υ f 3 = 0.5, f = 13 f 1 E Psi m = Gm ( 1+ ) Matrix E 6 = m = Psi υ m υ υ = 0.35 m υ 96
111 5.5 Boundary Conditions As stated earlier, the primary objective of the RVE model is to predict homogenized elastic properties of a lamina. Equations ( ) established a relation between the elastic properties of a homogenous composite material and the terms of stiffness matrix. FE based RVE model first evaluates the terms of stiffness matrix. From equation 5..1 it is clear that the stiffness matrix can be defined in terms of stresses if the volume average strains ε ij in the RVE are predefined. That means that if ε 1 = 1 and ε = ε 3 = γ 4 = γ 5 = γ 6 = 0 in equation 5..1 then C 11 = σ 1, C 1 = σ. Similarly other terms can be evaluated. However volume average strain is not the parameter that the user can control. Instead we can use applied strain ε 0 ij to induce a desired volume averaged strain averaged strain and the applied strain as [58] 0 In the RVE six components of strain ( ij ) displacement components. ε ij in the RVE. This follows from the relation between the volume 1 ε dv 0 ij = ε V ij = ε ij (5.5.1) V ε use the following boundary conditions on the 0 a x a u i ( a, x, y) u ( a, x, y) a 1 i = ε 1 1 i1 a y a a z a 1 1 u i ( z, a, y) u ( z, a, y) a i = ε i a y a a z a (,, ) (,, ) 1 1 u i z x a u z x a a 3 i = ε 3 3 i3 a x a (5.5.) (5.5.3) (5.5.4) 97
112 where i, j = 1..3 and the superscript ( ) 0 indicates the applied strain. The left hand of the equations ( ) indicates the relative displacement between the two opposite faces of the RVE including edges and vertices. Furthermore, aε 0 ij is the displacement necessary to enforce the j strain 0 ε ij over a distance a j. Fig is a representation of the RVE block without the distinction between fiber and matrix components. It shows the coordinates of the sides of the RVE and acts as a visual aid in understanding the application of BCs using the equations ( ). As shown in the Fig Z represents the 1 (fiber direction) and X and Y represent and 3 directions respectively. a +a (a1, x, y) +a3 (z, a, y) (+a1, x, y) Y (3) X () (z, +a, y) Z (1) a3 (z, x, a3) +a1 a1 Fig Coordinates of six faces on the RVE block To determine the coefficients of stiffness matrix, the boundary conditions were applied on the RVE in three stages. Each stage exposed the RVE to a particular boundary condition. This three stage condition is true for a transversely isotropic body. This is because in three stages all the necessary coefficients of stiffness matrix are obtained which are necessary to 98
113 find the elastic properties of the composite material. The coefficients of the stiffness matrix in equation 5..1 were evaluated column wise. The procedure of evaluating the stiffness coefficients in each of the six columns is explained in following steps. First Column To determine components in the first column of equation 5..1, following strain was applied to the RVE in fiber direction (Zdirection). ε 0 = 1 and ε = ε = 3 γ = 4 γ = γ = (5.5.5) 6 Equation can be applied in terms of terms of DOF as u1 ( a, x, y) u1( a, x, y) = a u ( a, x, y) u ( a, x, y) = 0 a y a, a x a 1 1 u3( a, x, y) u3( a, x, y) = (5.5.6) U 1 (a 1, x, y) Y (3) X () Z (1) U 1 (a 1, x, y) Fig Displacement BC on faces (a 1, x, y) and (a 1, x, y) As shown in Fig unit strain is applied between the faces (a 1, x, y) and (a 1, x, y) of the RVE in Z direction (1 direction) while the relative X, Y DOF between the two faces have been 99
114 constrained to prevent rigid body rotation. From equation the displacement necessary to cause this strain in fiber direction is a 1. The FE model generates the first set of stiffness coefficients as 7 C 11 = σ 1 = σ z (5.5.7) C 1 = σ = σ x (5.5.8) Second Column For the second column of the stiffness matrix of equation 5..1 ε 0 1 and = ε 1 = ε 3 = γ 4 = γ 5 = γ 6 = 0 (5.5.9) Equation can be applied in terms of terms of DOF as u ( z, a, y) u ( z, a, y) = u ( z, a, y) u ( z, a, y) = a a z a, a y a u ( z, a, y) u ( z, a, y) = (5.5.10) U (z,a, y) Y (3) X () U (z, +a, y) Z (1) Fig Displacement BC on faces (z,a, y) and (z, +a, y) 7 ANSYS TM 10.0 program used for generating the volume averaged stresses for the RVE has been be explained in sec
115 As shown in Fig unit strain is applied between the faces (z, a, y) and (z, +a, y) of the RVE. From equation the displacement necessary to cause this strain in X direction is a. The stiffness coefficient that is needed from this column is C = σ = σx (5.5.11) C 3 = σ 3 = σ y (5.5.1) Third Column From equation 5..1, all three stiffness matrix coefficients have been obtained from first and second column. Thus there is no need to evaluate any term from this column. Fourth Column From equation 5..1 it is evident that in the fourth column of the stiffness matrix only one nonzero term (C 44 ) exists which can be evaluated as ( ) 1 C 44 = C C 33 (5.5.16) Fifth Column Again from equation 5..1 it is clear that only term C 55 is nonzero. Also, relationship between C 55 and C 66 for transversely isotropic material is C 55 = C 66 (5.5.17) 101
116 Sixth Column In order to evaluate C 66 in the sixth and last column of the stiffness matrix the following relation should be satisfied γ 0 1 and = ε 1 = ε = ε = γ 4 = γ 5 = 0 (5.5.18) But γ 6 = ε 1 + ε 1 = 1 (5.5.19) and ε = ε 1 (5.5.0) From and it implies that 0 1 ε = should be applied between faces (a 1 1, x, y) and (a 1, x, y) and other half should be applied between (z, a, y) and (z, a, y). This can be simply understood from the equation 5.5. and equation in which i takes values from In equation 5.5. when ε = is applied while keeping ε 1 11 = ε 31 = 0 we get u1 ( a, x, y) u1( a, x, y) = u ( a, x, y) u ( a, x, y) = a a x a, a y a 1 1 u3( a, x, y) u3( a, x, y) = (5.5.1) Similarly, using equation the other half of the inplane shear 0 1 ε 1 = is applied between 0 0 faces (z, a, y) and (z, a, y) while keeping ε = ε 3 = 0 we get u1 ( a, x, y) u1( a, x, y) = a 1 1 u ( a, x, y) u ( a, x, y) = 0 a x a, a y a 1 1 u3( a, x, y) u3( a, x, y) = (5.5.) 10
117 The net effect of equations and 5.5. is shown in Fig The FE model under boundary conditions and 5.5. resulted in pure inplane shear and provided C 66 as C 66 = σ = σ (5.5.3) 6 xz Fig shows the faces over which the shear is applied. The top view of the RVE block in Fig shows the shear effect in 1 plane. Top Face (a1, x, y) Top Face Y (3) x () (z, a, y) Z (1) X () (z, +a, y) z (1) (+a1, x, y) Fig Displacement BC on faces (+a 1, x, y) and (a 1, x, y) and faces (z, a, y) and (z, +a, y). Top face showing the shear effect in 1 plane. 103
118 5.6 FE Code Implementation Fig Flow chart for the RVE model The flowchart in Fig lists the steps for proceeding with the Finite Element model of the RVE. First of all, the parameters  fiber volume fraction ( ν f ) and fiber diameter ( d f ) fixed. As explained in section 5.3 the RVE dimensions (a 1, a, a 3 ) were evaluated using ν f and 104 were
119 d f. Ansys TM 10.0 FEA package was used for the numerical modeling of the RVE. Using a 1, a, a 3 and d f, the geometry of the RVE model was created. The material model parameters were set. As shown in Table orthotropic properties were selected for the fiber and isotropic properties were selected for the matrix. Fig.5.6. Full model of RVE Solid 186 was used for generating the mesh of the RVE. Fig.5.6. shows the FE mesh of the RVE model. Solid 186 is a 0 noded brick element with layered and nonlayered option. For the RVE model, the nonlayered option was chosen by setting Keyopt (3) = 0 in the element settings. After mesh generation the set of boundary conditions as described in sections ( ) were applied. The CE command in the ANSYS Parametric Design Language (APDL) was used for defining BCs using degrees of freedom. After invoking the CE command the user is prompted for the input: CE, NEQN, CONST, NODE1, Lab1, NODE, Lab, NODE3, Lab3. 105
Openhole compressive strength prediction of CFRP composite laminates
Openhole compressive strength prediction of CFRP composite laminates O. İnal 1, A. Ataş 2,* 1 Department of Mechanical Engineering, Balikesir University, Balikesir, 10145, Turkey, inal@balikesir.edu.tr
More informationFINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Ever J. Barbero Department of Mechanical and Aerospace Engineering West Virginia University USA CRC Press Taylor &.Francis Group Boca Raton London New York
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationStress, Strain Stress strain relationships for different types of materials Stress strain relationships for a unidirectional/bidirectional lamina
Chapter 2 Macromechanical Analysis of a Lamina Stress, Strain Stress strain relationships for different types of materials Stress strain relationships for a unidirectional/bidirectional lamina Islamic
More informationINTERNATIONAL JOURNAL OF APPLIED ENGINEERING RESEARCH, DINDIGUL Volume 2, No 1, 2011
Interlaminar failure analysis of FRP cross ply laminate with elliptical cutout Venkateswara Rao.S 1, Sd. Abdul Kalam 1, Srilakshmi.S 1, Bala Krishna Murthy.V 2 1 Mechanical Engineering Department, P. V.
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More information9 Strength Theories of Lamina
9 trength Theories of Lamina 9 TRENGTH O ORTHOTROPIC LAMINA or isotropic materials the simplest method to predict failure is to compare the applied stresses to the strengths or some other allowable stresses.
More informationEffect of Thermal Stresses on the Failure Criteria of Fiber Composites
Effect of Thermal Stresses on the Failure Criteria of Fiber Composites Martin Leong * Institute of Mechanical Engineering Aalborg University, Aalborg, Denmark Bhavani V. Sankar Department of Mechanical
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationThe Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints
, June 30  July 2, 2010, London, U.K. The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints O. Aluko, and Q. Mazumder Abstract An analytical model was developed
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationCoupling of plasticity and damage in glass fibre reinforced polymer composites
EPJ Web of Conferences 6, 48 1) DOI: 1.151/epjconf/1648 c Owned by the authors, published by EDP Sciences, 1 Coupling of plasticity and damage in glass fibre reinforced polymer composites R. Kvale Joki
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationCapability Assessment of Finite Element Software in Predicting the Last Ply Failure of Composite Laminates
Available online at www.sciencedirect.com Procedia Engineering 41 (2012 ) 1647 1653 International Symposium on Robotics and Intelligent Sensors 2012 (IRIS 2012) Capability Assessment of Finite Element
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationFinite ElementBased Failure Models for Carbon/Epoxy Tape Composites
Finite ElementBased Failure Models for Carbon/Epoxy Tape Composites A Master Thesis Presented to The Academic Faculty by Guillaume Seon In Partial Fulfillment of the Requirements for the Degree Master
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationFracture Mechanics, Damage and Fatigue: Composites
University of Liège Aerospace & Mechanical Engineering Fracture Mechanics, Damage and Fatigue: Composites Ludovic Noels Computational & Multiscale Mechanics of Materials CM3 http://www.ltascm3.ulg.ac.be/
More informationDevelopment of a Progressive Failure Model for Notched Woven Composite Laminates. Daniel Christopher Munden
Development of a Progressive Failure Model for Notched Woven Composite Laminates Daniel Christopher Munden Thesis submitted to the faculty of the Virginia Polytechnic Institute and State University in
More informationTHE MUTUAL EFFECTS OF SHEAR AND TRANSVERSE DAMAGE IN POLYMERIC COMPOSITES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS THE MUTUAL EFFECTS OF SHEAR AND TRANSVERSE DAMAGE IN POLYMERIC COMPOSITES L.V. Smith 1 *, M. Salavatian 1 1 School of Mechanical and Materials
More informationMODELING OF THE BEHAVIOR OF WOVEN LAMINATED COMPOSITES UNTIL RUPTURE
MODELING OF THE BEHAVIOR OF WOVEN LAMINATED COMPOSITES UNTIL RUPTURE Jean Paul Charles, Christian Hochard,3, Pierre Antoine Aubourg,3 Eurocopter, 375 Marignane cedex, France Unimeca, 6 rue J. Curie, 3453
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationMulti Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala
Multi Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala Abstract: FRP laminated composites have been extensively used in Aerospace and allied industries
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationComparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost
Comparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost 1 Mihir A. Mehta, 2 Satyen D. Ramani 1 PG Student, Department
More informationSamantha Ramirez, MSE. Stress. The intensity of the internal force acting on a specific plane (area) passing through a point. F 2
Samantha Ramirez, MSE Stress The intensity of the internal force acting on a specific plane (area) passing through a point. Δ ΔA Δ z Δ 1 2 ΔA Δ x Δ y ΔA is an infinitesimal size area with a uniform force
More informationModeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites
Modeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites H.E.Pettermann 1, C.Schuecker 1, D.H.Pahr 2, F.G.Rammerstorfer 2 1 Austrian Aeronautics
More informationACDC. User Manual. Ver. 1.0
ACDC User Manual Ver. 1.0 Centre Composite December 2016 ACDC, Ver. 1.0 User Manual Centre Composite, 2016 (software@composite.lv) Table of Contents Introduction... 1 System requirements... 1 Theoretical
More informationMechanical Properties of Materials
Mechanical Properties of Materials Strains Material Model Stresses Learning objectives Understand the qualitative and quantitative description of mechanical properties of materials. Learn the logic of
More informationMechanical and Thermal Properties of Coir Fiber Reinforced Epoxy Composites Using a Micromechanical Approach
Mechanical and Thermal Properties of Coir Fiber Reinforced Epoxy Composites Using a Micromechanical Approach Sandhyarani Biswas Department of Mechanical Engineering, N.I.T Rourkela, INDIA Abstract: Nowadays,
More informationStrength of GRPlaminates with multiple fragment damages
Strength of GRPlaminates with multiple fragment damages S. Kazemahvazi, J. Kiele, D. Zenkert Kungliga Tekniska Högskolan, KTH 100 44 Stockholm, Sweden sohrabk@kth.se SUMMARY The strength of glass fibre
More informationAn ElastoViscoPlastic Multiscale Model for Fibrous Unidirectional Composite Materials
An ElastoViscoPlastic Multiscale Model for Fibrous Unidirectional Composite Materials by Shari Lynn King A thesis presented to the University of Waterloo in fulfillment of the thesis requirement for
More informationProgressive Failure Analysis Methodology for Laminated Composite Structures
NASA/TP9990907 Progressive Failure Analysis Methodology for Laminated Composite Structures David W. Sleight Langley Research Center, Hampton, Virginia March 999 The NASA STI Program Office... in Profile
More informationMODELING DYNAMIC FRACTURE AND DAMAGE IN A FIBERREINFORCED COMPOSITE LAMINA WITH PERIDYNAMICS
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Mechanical & Materials Engineering Faculty Publications Mechanical & Materials Engineering, Department of 011 MODELING DYNAMIC
More informationME 7502 Lecture 2 Effective Properties of Particulate and Unidirectional Composites
ME 75 Lecture Effective Properties of Particulate and Unidirectional Composites Concepts from Elasticit Theor Statistical Homogeneit, Representative Volume Element, Composite Material Effective Stress
More informationComposites Design and Analysis. Stress Strain Relationship
Composites Design and Analysis Stress Strain Relationship Composite design and analysis Laminate Theory Manufacturing Methods Materials Composite Materials Design / Analysis Engineer Design Guidelines
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of Materials Science and Engineering A 6 () 354 doi:.765/663/6..5 D DAVID PUBLISHING Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K * and V V Subba Rao Faculty
More informationPREDICTION OF OUTOFPLANE FAILURE MODES IN CFRP
PREDICTION OF OUTOFPLANE FAILURE MODES IN CFRP R. R. Pinto 1, P. P. Camanho 2 1 INEGI  Instituto de Engenharia Mecanica e Gestao Industrial, Rua Dr. Roberto Frias, 4200465, Porto, Portugal 2 DEMec,
More informationFailure analysis of serial pinned joints in composite materials
Indian Journal of Engineering & Materials Sciences Vol. 18, April 2011, pp. 102110 Failure analysis of serial pinned joints in composite materials Alaattin Aktaş* Department of Mechanical Engineering,
More informationSIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO MULTIPLE LOADING WITH MEMBRANEFLEXION COUPLING EFFECTS
VOL. 5, NO. 4, APRIL 010 ISSN 18196608 006010 Asian Research Publishing Network (ARPN). All rights reserved. SIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO
More informationComposite models 30 and 131: Ply types 0 and 8 calibration
Model calibration Composite BiPhase models 30 and 3 for elastic, damage and failure PAMCRASH material model 30 is for solid and 3 for multilayered shell elements. Within these models different ply types
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More informationImpact and Crash Modeling of Composite Structures: A Challenge for Damage Mechanics
Impact and Crash Modeling of Composite Structures: A Challenge for Damage Mechanics Dr. A. Johnson DLR Dr. A. K. Pickett ESI GmbH EUROPAM 99 Impact and Crash Modelling of Composite Structures: A Challenge
More informationDAMAGE MECHANICS MODEL FOR OFFAXIS FATIGUE BEHAVIOR OF UNIDIRECTIONAL CARBON FIBERREINFORCED COMPOSITES AT ROOM AND HIGH TEMPERATURES
DAMAGE MECHANICS MODEL FOR OFFAXIS FATIGUE BEHAVIOR OF UNIDIRECTIONAL CARBON FIBERREINFORCED COMPOSITES AT ROOM AND HIGH TEMPERATURES M. Kawai Institute of Engineering Mechanics University of Tsukuba,
More informationPLY LEVEL UNCERTAINTY EFFECTS ON FAILURE OF COMPOSITE
7th European Workshop on Structural Health Monitoring July 811, 2014. La Cité, Nantes, France More Info at Open Access Database www.ndt.net/?id=17206 PLY LEVEL UNCERTAINTY EFFECTS ON FAILURE OF COMPOSITE
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationMAE 322 Machine Design. Dr. Hodge Jenkins Mercer University
MAE 322 Machine Design Dr. Hodge Jenkins Mercer University What is this Machine Design course really about? What you will learn: How to design machine elements 1) Design so they won t break under varying
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationTvestigated using the quadratic form of the TsaiWu strength theory [I].
Evaluation of Strength the TensorPolynomial Theory for Wood J. Y. L IU* Forest Products Laboratory, Forest Service U.S. Department of Agriculture, Madison, Wisconsin 53705 (Received October 10, 1983) (Revised
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationGetting Started with Composites Modeling and Analysis
Getting Started with Composites Modeling and Analysis IN THIS WEBINAR: PRESENTED BY: Orthotropic materials and how to define them Composite Laminate properties and modeling Composite failure theories and
More informationSKINSTRINGER DEBONDING AND DELAMINATION ANALYSIS IN COMPOSITE STIFFENED SHELLS
SKINSTRINER DEBONDIN AND DELAMINATION ANALYSIS IN COMPOSITE STIFFENED SHELLS R. Rikards, K. Kalnins & O. Ozolinsh Institute of Materials and Structures, Riga Technical University, Riga 1658, Latvia ABSTRACT
More information[5] Stress and Strain
[5] Stress and Strain Page 1 of 34 [5] Stress and Strain [5.1] Internal Stress of Solids [5.2] Design of Simple Connections (will not be covered in class) [5.3] Deformation and Strain [5.4] Hooke s Law
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationFracture Behaviour of FRP CrossPly Laminate With Embedded Delamination Subjected To Transverse Load
Fracture Behaviour of FRP CrossPly Laminate With Embedded Delamination Subjected To Transverse Load Sriram Chintapalli 1, S.Srilakshmi 1 1 Dept. of Mech. Engg., P. V. P. Siddhartha Institute of Technology.
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationMultiscale Approach to Damage Analysis of Laminated Composite Structures
Multiscale Approach to Damage Analysis of Laminated Composite Structures D. Ivančević and I. Smojver Department of Aeronautical Engineering, Faculty of Mechanical Engineering and Naval Architecture, University
More informationSTRESS DISTRIBUTION AND STRENGTH PREDICTION OF COMPOSITE LAMINATES WITH MULTIPLE HOLES BRIAN ESP. Presented to the Faculty of the Graduate School of
STRESS DISTRIBUTION AND STRENGTH PREDICTION OF COMPOSITE LAMINATES WITH MULTIPLE HOLES by BRIAN ESP Presented to the Faculty of the Graduate School of The University of Texas at Arlington in Partial Fulfillment
More informationCrashworthiness of composite structures: Experiment and Simulation
Crashworthiness of composite structures: Experiment and Simulation Francesco Deleo, Bonnie Wade and Prof. Paolo Feraboli (UW) Dr. Mostafa Rassaian (Boeing R&T) JAMS 2010 The Joint Advanced Materials and
More informationDerivation of the stress concentrations at holes in orthotropic plates using thermoelastic stress analysis
Derivation of the stress concentrations at holes in orthotropic plates using thermoelastic stress analysis S. Quinn, S. Sambasivam and J.M. DulieuBarton School of Engineering Sciences, University of Southampton,
More informationModelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations
Modelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations W. Van Paepegem *, I. De Baere and J. Degrieck Ghent
More information5. STRESS CONCENTRATIONS. and strains in shafts apply only to solid and hollow circular shafts while they are in the
5. STRESS CONCENTRATIONS So far in this thesis, most of the formulas we have seen to calculate the stresses and strains in shafts apply only to solid and hollow circular shafts while they are in the elastic
More informationAnalysis of Composite Pressure Vessels
Analysis of Composite Pressure Vessels Reza Mohammadzadeh Gheshlaghi 1 Mohammad Hassan Hojjati Hamid Reza Mohammadi Daniali 3 1 Engineering Research Centre, Tabriz, Iran,3 Department of Mechanical Engineering,
More informationINITIATION AND PROPAGATION OF FIBER FAILURE IN COMPOSITE LAMINATES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS INITIATION AND PROPAGATION OF FIBER FAILURE IN COMPOSITE LAMINATES E. Iarve 1,2*, D. Mollenhauer 1, T. Breitzman 1, K. Hoos 2, M. Swindeman 2 1
More informationCalculation of Damagedependent Directional Failure Indices from the TsaiWu Static Failure Criterion
Van Paepegem, W. and Degrieck, J. (3. alculation of Damagedependent Directional Failure Indices from the saiwu Static Failure riterion. omposites Science and echnology, 63(, 353. alculation of Damagedependent
More informationNumerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints
THEORETICAL & APPLIED MECHANICS LETTERS 1, 041005 (2011) Numerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints M. R. Khoshravan,
More informationMicromechanical analysis of FRP hybrid composite lamina for inplane transverse loading
Indian Journal of Engineering & Materials Sciences Vol. 15, October 2008, pp. 382390 Micromechanical analysis of FRP hybrid composite lamina for inplane transverse loading K Sivaji Babu a *, K Mohana
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationMECHANICS OF MATERIALS
CHATR Stress MCHANICS OF MATRIALS and Strain Axial Loading Stress & Strain: Axial Loading Suitability of a structure or machine may depend on the deformations in the structure as well as the stresses induced
More informationComposite Structures Modeling, FEA, Optimization and Diagnostics
Composite Structures Modeling, FEA, Optimization and Diagnostics Ratan Jha Mechanical and Aeronautical Engineering Clarkson University, Potsdam, NY Composite Laminate Modeling Refined Higher Order Displacement
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationON HOMOGENIZATION AND DEHOMOGENIZATION OF COMPOSITE MATERIALS. A Thesis. Submitted to the Faculty. Drexel University.
ON HOMOGENIZATION AND DEHOMOGENIZATION OF COMPOSITE MATERIALS A Thesis Submitted to the Faculty of Drexel University by Chang (Karen) Yan in partial fulfillment of the requirements for the degree of Doctor
More informationEXPLICIT DYNAMIC SIMULATION OF DROPWEIGHT LOW VELOCITY IMPACT ON CARBON FIBROUS COMPOSITE PANELS
EXPLICIT DYNAMIC SIMULATION OF DROPWEIGHT LOW VELOCITY IMPACT ON CARBON FIBROUS COMPOSITE PANELS Umar Farooq and Karl Gregory School of Built Environment and Department of Engineering, University of Bolton,
More informationModule 4: Behaviour of a LaminaeII. Learning Unit 1: M1. M4.1 Mechanics of Composites. M4.1.1 Introduction to Mechanics of Composites
Module 4: Behaviour of a LaminaeII Learning Unit 1: M1 M4.1 Mechanics of Composites M4.1.1 Introduction to Mechanics of Composites The relation between ply uniaxial strengths and constituent properties
More informationBEARING STRENGTH ASSESSMENT OF COMPOSITE MATERIAL THROUGH NUMERICAL MODELS
BEARING STRENGTH ASSESSMENT OF COMPOSITE MATERIAL THROUGH NUMERICAL MODELS Euler S. Dias*, Carlos A. Cimini Jr.* * Federal University of Minas Gerais, Dept. of Structural Engineering, Belo Horizonte 
More informationInternational Journal of Innovative Research in Science, Engineering and Technology Vol. 2, Issue 7, July 2013
ANALYSIS AND MITIGATION OF STRESS CONCENTRATION FACTOR OF A RECTANGULAR ISOTROPIC AND ORTHOTROPIC PLATE WITH CENTRAL CIRCULAR HOLE SUBJECTED TO INPLANE STATIC LOADING BY DESIGN OPTIMIZATION Shubhrata Nagpal
More informationNUMERICAL INVESTIGATION OF DELAMINATION IN LSHAPED CROSSPLY COMPOSITE BRACKET
NUMERICAL INVESTIGATION OF DELAMINATION IN LSHAPED CROSSPLY COMPOSITE BRACKET M.Gümüş a*, B.Gözlüklü a, D.Çöker a a Department of Aerospace Eng., METU, Ankara, Turkey *mert.gumus@metu.edu.tr Keywords:
More informationFinite element analysis of drilled holes in unidirectional composite laminates using failure theories
American Journal of Science and Technology 2014; 1(3): 101105 Published online May 30, 2014 (http://www.aascit.org/journal/ajst) Finite element analysis of drilled holes in unidirectional composite laminates
More informationCalibration and Experimental Validation of LSDYNA Composite Material Models by Multi Objective Optimization Techniques
9 th International LSDYNA Users Conference Optimization Calibration and Experimental Validation of LSDYNA Composite Material Models by Multi Objective Optimization Techniques Stefano Magistrali*, Marco
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationFailure Analysis of Unidirectional Composite Pinned Joints
217 IJEDR Volume, Issue 4 ISSN: 23219939 Failure Analysis of Unidirectional Composite Pinned Joints 1 Sai Ashok.M, 2 Mr. U. Koteswara Rao 1 Mtech Machine Design, 2 Associate Professor & Asst. COE 1
More informationFailure surface according to maximum principal stress theory
Maximum Principal Stress Theory (W. Rankin s Theory 1850) Brittle Material The maximum principal stress criterion: Rankin stated max principal stress theory as follows a material fails by fracturing
More informationME 243. Mechanics of Solids
ME 243 Mechanics of Solids Lecture 2: Stress and Strain Ahmad Shahedi Shakil Lecturer, Dept. of Mechanical Engg, BUET Email: sshakil@me.buet.ac.bd, shakil6791@gmail.com Website: teacher.buet.ac.bd/sshakil
More informationGeneric Strategies to Implement Material Grading in Finite Element Methods for Isotropic and Anisotropic Materials
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Engineering Mechanics Dissertations & Theses Mechanical & Materials Engineering, Department of Winter 1292011 Generic
More informationConstitutive Equations
Constitutive quations David Roylance Department of Materials Science and ngineering Massachusetts Institute of Technology Cambridge, MA 0239 October 4, 2000 Introduction The modules on kinematics (Module
More informationCOMPARISON OF COHESIVE ZONE MODELS USED TO PREDICT DELAMINATION INITIATED FROM FREEEDGES : VALIDATION AGAINST EXPERIMENTAL RESULTS
COMPARISON OF COHESIVE ZONE MODELS USED TO PREDICT DELAMINATION INITIATED FROM FREEEDGES : VALIDATION AGAINST EXPERIMENTAL RESULTS A. Uguen 1, L. Zubillaga 2, A. Turon 3, N. Carrère 1 1 Laboratoire Brestois
More informationLecture 8. Stress Strain in Multidimension
Lecture 8. Stress Strain in Multidimension Module. General Field Equations General Field Equations [] Equilibrium Equations in Elastic bodies xx x y z yx zx f x 0, etc [2] Kinematics xx u x x,etc. [3]
More informationMICROMECHANICAL ANALYSIS OF FRP COMPOSITES SUBJECTED TO LONGITUDINAL LOADING
MICROMECHANICAL ANALYSIS OF FRP COMPOSITES SUBJECTED TO LONGITUDINAL LOADING N. Krishna Vihari 1, P. Phani Prasanthi 1, V. Bala Krishna Murthy 2* and A. Srihari Prasad 3 1 Mech. Engg. Dept., P. V. P. Siddhartha
More informationAn orthotropic damage model for crash simulation of composites
High Performance Structures and Materials III 511 An orthotropic damage model for crash simulation of composites W. Wang 1, F. H. M. Swartjes 1 & M. D. Gan 1 BU Automotive Centre of Lightweight Structures
More informationPressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials
Pressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials Pressure Vessels: In the previous lectures we have discussed elements subjected
More informationIJSER 1. INTRODUCTION. M.Elhadary
1591 A new failure criterion for GRP composite materials subjected to inphase and outofphase biaxial fatigue loading under different stress ratios M.Elhadary Abstract this studying the fatigue behavior
More information3.22 Mechanical Properties of Materials Spring 2008
MIT OpenCourseWare http://ocw.mit.edu 3.22 Mechanical Properties of Materials Spring 2008 For information about citing these materials or our Terms of Use, visit: http://ocw.mit.edu/terms. Quiz #1 Example
More informationModule4. Mechanical Properties of Metals
Module4 Mechanical Properties of Metals Contents ) Elastic deformation and Plastic deformation ) Interpretation of tensile stressstrain curves 3) Yielding under multiaxial stress, Yield criteria, Macroscopic
More informationEVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS T. Kurashiki 1 *, Y. Matsushima 1, Y. Nakayasu
More informationDYNAMIC FAILURE ANALYSIS OF LAMINATED COMPOSITE PLATES
Association of Metallurgical Engineers of Serbia AMES Scientific paper UDC:669.1419:628.183=20 DYNAMIC FAILURE ANALYSIS OF LAMINATED COMPOSITE PLATES J. ESKANDARI JAM 1 and N. GARSHASBI NIA 2 1 Aerospace
More informationSEMM Mechanics PhD Preliminary Exam Spring Consider a twodimensional rigid motion, whose displacement field is given by
SEMM Mechanics PhD Preliminary Exam Spring 2014 1. Consider a twodimensional rigid motion, whose displacement field is given by u(x) = [cos(β)x 1 + sin(β)x 2 X 1 ]e 1 + [ sin(β)x 1 + cos(β)x 2 X 2 ]e
More information